* Your assessment is very important for improving the workof artificial intelligence, which forms the content of this project
Download pp-03-25-new dots.qxd
Document related concepts
pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 507 LITHIUM OXIDE 507 LITHIUM OXIDE [12057-24-8] Formula: Li2O; MW 29.88 Synonym: lithium monoxide Uses Lithium oxide in its highly porous sintered form is used as an absorbent for carbon dioxide. Physical Properties White cubic crystals; refractive index 1.644; density 2.013 g/cm3; melts at 1,570°C; dissolves and decomposes in water (6.67 g/100g at 0°C and 10.02 g/100g at 100°C). Thermochemical Properties ∆Hƒ° (cry) ∆Hƒ° (gas) ∆Gƒ° (cry) ∆Gƒ° (gas) S° (cry) S° (gas) Cρ (cry) Cρ (gas) –142.91 kcal/mol –38.4 kcal/mol –134.13 kcal/mol –43.3 kcal/mol 8.98 cal/degree mol 55.30 cal/degree mol 12.93 cal/degree mol 11.91 cal/degree mol Preparation Lithium oxide is prepared by heating lithium metal in dry oxygen above 100°C: 4Li + O2 heat → 2Li2O Another method of preparation that yields pure lithium oxide involves thermal decomposition of lithium peroxide: 2Li2O2 heat → 2Li2O + O2 Also, the oxide can be produced by heating the pure lithium hydroxide at 800°C in a vacuum: 2LiOH 800°C −−−−−→ Li2O + H2O vacuum Reactions Lithium oxide absorbs carbon dioxide forming lithium carbonate: pp-03-25-new dots.qxd 508 10/23/02 2:38 PM Page 508 LITHIUM SULFATE Li2O + CO2 → Li2CO3 The oxide reacts slowly with water forming lithium hydroxide: Li2O + H2O → 2LiOH There is no reaction with oxygen at high temperature or high pressure to form any peroxide or higher oxide. The oxide reacts with acids forming lithium salts. Analysis Elemental composition: Li 46.45%, O 53.55%. The oxide may be identified from its physical properties and characterized by x-ray analysis. Lithium composition in the oxide may be determined by analyzing the nitric acid extract by AA or ICP (See Lithium). LITHIUM SULFATE [10377-48-7] Formula: Li2SO4; MW 109.94 Also forms a stable monohydrate, Li2SO4•H2O [10102-25-7] Uses Lithium sulfate is used in making a special type of high strength glass. It also is used in medicine as an antidepressant. Physical Properties Colorless monoclinic or hexagonal crystals; transforms to cubic form at 500°C; refractive index 1.465; density 2.221 g/cm3; sublimes at 845°C; soluble in water, solubility decreases with an increase in temperature (26.1 and 23.2 g at 0 and 100°C, respectively); insoluble in absolute ethanol and acetone. The monohydrate constitutes colorless monoclinic crystals; refractive index 1.465; density 2.06 g/cm3; loses water of crystallization at 130°C; soluble in water, (more soluble than the anhydrous salt (34.9 and 29.2 g/100g at 25 and 100°C), respectively; insoluble in acetone and pyridine. Thermochemical Properties ∆Hƒ° (Li2SO4) ∆Hƒ° (Li2SO4•H2O) ∆Hƒ° (Li SO4 )(aq) ∆Gƒ° (Li2SO4) ∆Gƒ° (Li2SO4•H2O) ∆Gƒ° (Li SO4)(aq) S° (Li2SO4) S° (Li2SO4•H2O) S° (Li SO4)(aq) –343.33 kcal/mol –414.80 kcal/mol –350.44 kcal/mol –315.91 kcal/mol –374.2 kcal/mol –318.18 kcal/mol 27.5 cal/degree mol 39.1 cal/degree mol 11.3 cal/degree mol pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 509 LUTETIUM Cρ (Li2SO4) Cρ (Li2SO4•H2O) 509 28.10 cal/degree mol 36.1 cal/degree mol Preparation Lithium sulfate is prepared by neutralization of lithium hydroxide or lithium carbonate with sulfuric acid followed by crystallization: 2LiOH + H2SO4 → Li2SO4 + H2O Li2CO3 + H2SO4 → Li2SO4 + CO2 + H2O The product obtained from crystallization in a concentrated solution is the monohydrate, Li2SO4•H2O. Anhydrous salt is obtained by heating the monohydrate in a vacuum. Analysis Elemental composition (anhydrous Li2SO4): Li 12.63%, S 29.12%, O 59.28%. The waters of crystallization may be determined by gravimetry. Lithium may be analyzed in a dilute aqueous solution by AA or ICP (See Lithium), while sulfate may be measured by ion chromatography. LUTETIUM [7439-94-3] Symbol Lu; atomic number 71; atomic weight 174.97; a lanthanide series element; an ƒ-block inner-transition metal; electron configuration [Xe]4ƒ145d16s2; valence +3; atomic radius (coordination number 12) 1.7349Å; ionic radius (Lu3+) 0.85Å; two naturally-occurring isotopes: Lu-176 (97.1%) and Lu-175(2.59%); Lu-172 is radioactive with a half-life of 4x1010 years (beta-emission); several artificial isotopes known, that have mass numbers 155, 156, 167–174, 177–180. History, Occurrence, and Uses Lutetium was independently discovered by Urbain and von Welsbach in 1907. The element was named after Lutetia, the ancient name for Paris. The metal also is known as cassiopeium in Germany. Lutetium occurs in nature in small amounts in yttrium-containing minerals. It is found in xenotime, precambrian granites, and North American shales. It also exists at 0.001% in monazite, from which the metal is produced commercially. Lutetium has very little commercial application. The metal emits beta particles after thermal neutron activation, and is used to catalyze organic reactions. Physical Properties Silvery-white metal; hexagonal close-packed structure; density 9.84 g/cm3; melts at 1,663°C; vaporizes at 3,402°C; electrical resistivity 59 microhm-cm; slightly paramagnetic; thermal neutron cross section 108 barns; soluble in acids. pp-03-25-new dots.qxd 510 10/23/02 2:38 PM Page 510 MAGNESIUM Thermochemical Properties ∆Hƒ° (cry) ∆Hƒ° (gas) ∆Gƒ° (gas) S° (cry) S° (gas) Cρ (cry) Cρ (gas) ∆Hfus (cry) ∆Hvap (cry) 0.0 102.2 kcal/mol 96.7 kcal/mol 12.18 cal/degree mol 44.14 cal/degree mol 6.42 cal/degree mol 4.99 cal/degree mol 4.60 kcal/mol 102.2 kcal/mol\ Production Lutetium is produced commercially from monazite. The metal is recovered as a by-product during large-scale extraction of other heavy rare earths (See Cerium, Erbium, Holmium). The pure metal is obtained by reduction of lutetium chloride or lutetium fluoride by a alkali or alkaline earth metal at elevated temperatures; 2LuCl3 + 3Ca elevated temperatur e → 2Lu + 3CaCl2 Chemical Properties In aqueous media lutetium occurs as tripositive Lu3+ ion. All its compounds are in +3 valence state. Aqueous solutions of all its salts are colorless, while in dry form they are white crystalline solids. The soluble salts such as chloride, bromide, iodide, nitrate, sulfate and acetate form hydrates upon crystallization. The oxide, hydroxide, fluoride, carbonate, phosphate, and oxalate of the metal are insoluble in water. The metal dissolves in acids forming the corresponding salts upon evaporation of the solution and crystallization. Analysis The metal may be analyzed by AA, ICP-AES, ICP/MS, x-ray fluorescence and other instrumental techniques. MAGNESIUM [7439-95-4] Symbol Mg; atomic number 12; atomic weight 24.305; a Group II A (Group 2) alkaline-earth metal; atomic radius 1.60Å; ionic radius (Mg2+) 0.72Å; atomic volume 14.0 cm3/mol; electron configuration [Ne]3s2; valence +2; ionization potential 7.646 and 15.035eV for Mg+ and Mg2+, respectively; three natural isotopes: Mg-24(78.99%), Mg-25(10.00%), Mg-26(11.01%). History, Occurrence and Uses Magnesium was discovered by Davy in 1808. He produced an amalgam of magnesium both by chemical and electrolytic methods. Metallic mercury was pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 511 MAGNESIUM 511 used in both methods. In the chemical method, Davy passed potassium vapors over magnesia at red heat and extracted the ‘new element’ with mercury. In the electrolytic reduction, magnesium sulfate was electrolyzed using a mercury cathode. Both the methods yielded the amalgam of the new element. Magnesium in the metallic form was first isolated by French chemist Bussy in 1828 by heating magnesium chloride with potassium metal at elevated temperatures. Faraday in 1833 produced metallic magnesium by electrolysis of magnesium chloride. Magnesium is probably one of the most common metals distributed in nature, constituting about 2.4% of the earth’s crust. The metal, however, does not occur in nature in elemental form. The principal minerals are dolomite [CaMg(CO3)2], magnesite MgCO3; carnallite KCl•MgCl2•6H2O, and silicate materials, such as talc Mg3(Si4O10)(OH)2 and asbestos H4Mg3Si2O9. Magnesium also is found in seawater, natural underground brines and salt deposits. Its concentration in sea water is 1,350 mg/L. Magnesium also occurs in all plants. Its porphyrin complex, chlorophyll, is essential for photosynthesis. It also is an essential nutrient element for humans. The dietary requirement for adults is about 300 mg per day. Magnesium metal and its alloys have numerous uses in chemical, electrochemical, metallurgy, and electronic industries. Its thermal and electrical properties, lightness, and ease of fabrication into useful shapes make it an attractive choice in industrial applications. The metal is alloyed with aluminum for various structural uses. Its alloys with zinc, copper, nickel, lead, zirconium and other metals have many uses too. Magnesium alloys are used in automobile parts, aircraft, missiles, space vehicles, ship hulls, underground pipelines, memory discs, machine tools, furniture, lawn mowers, ladders, toys, and sporting goods. It also is used in making small and lightweight dry cell batteries. Chemical applications of magnesium include its use as a reducing agent, to prepare Grignard reagent for organic syntheses, and to purify gases. Magnesium also is used in blasting compositions, explosive sensitizers, incendiaries, signal flares, and pyrotechnics. Magnesium salts have numerous uses. They are discussed individually. Physical Properties Silvery-white metal; close-packed hexagonal structure; density 1.74 g/cm3 at 20°C, 1.57 g/cm3 at 650°C (liquid melt); melts at 650°C; vaporizes at 1,090°C; vapor pressure 5 torr at 678°C and 20 torr at 763°C; electrical resistivity 4.46 microhm-cm at 20°C, 28.0 microhm-cm at 650°C (liquid melt); surface tension 563 dynes/cm at 681°C; modulus of elasticity 6.5x106 lb/sq in; Poisson’s ratio 0.35; thermal neutron absorption cross section 0.059 barn; soluble in dilute acids. Thermochemical Properties ∆Hƒ° (cry) ∆Hƒ°° (gas) ∆Gƒ° (gas) S° (cry) 0.0 35.16 kcal/mol 26.89 kcal/mol 7.82 cal/degree mol pp-03-25-new dots.qxd 512 10/23/02 2:38 PM Page 512 MAGNESIUM S° (gas) Cρ (cry) Cρ (gas) ∆Hfus ∆Hvap Thermal conductivity at 27°C Coefficeint of linear expansion (20–100°C) 35.52 cal/degree mol 5.95 cal/degree mol 4.97 cal/degree mol 2.03 kcal/mol 49.9 kcal/mol 1.56 W/cm. K 26.1x10–6/°C Production Although many commercial processes have been developed since the first electrolytic isolation of Mg metal by Davy and Faraday, and Bussy, by chemical reduction, the principles of the manufacturing processes have not changed. At present, the metal is most commonly manufactured by electrolytic reduction of molten magnesium chloride, in which chlorine is produced as a by-product. In chemical reduction processes, the metal is obtained by reduction of magnesium oxide, hydroxide, or chloride at elevated temperatures. All the magnesium produced in the world currently is derived from its minerals dolomite and carnallite, as well as from the underground brines and seawaters. In most processes, magnesium is recovered from its mineral or brine either as magnesium chloride or converted to the latter for electrolytic production. Many subterranean brines are very rich in magnesium chloride, often containing about 11% MgCl2. Sodium and calcium chlorides are the other two major components (c.12% NaCl and 2% CaCl2) in such brines. Solar evaporation of the brine solution and repeated heating increases the MgCl2 concentration in the brine to above 25% at which the solubility of NaCl significantly decreases and it can be filtered out. Repeated spray drying and purification by chlorination yields anhydrous magnesium chloride. Magnesium chloride produced from dolomite for electrolysis involves a series of steps that include calcinations of the mineral to oxide and then conversion to magnesium hydroxide, neutralization of the hydroxide with hydrochloric acid to form hydrated chloride, addition of sulfuric acid to separate out calcium as its insoluble sulfate, and dehydration of the hydrated salt to yield anhydrous MgCl2. Similar steps are also followed to obtain the metal from seawater. The average concentration of magnesium ion in seawater is about 1,200 mg/L, thus making ocean water an enormous source of magnesium. Magnesium is precipitated as hydroxide by treatment with lime in an agitated flocculator: MgCl2 + Ca(OH)2 → Mg(OH)2 + CaCl2 The insoluble Mg(OH)2 is filtered off and the seawater containing calcium chloride is returned to the sea. The hydroxide is then neutralized with hydrochloric acid. Evaporation of the solution yields hexahydrate, MgCl2•6H2O. The hexahydrate is either fully dehydrated to anhydrous MgCl2 by heating in dryers or partially dehydrated to monohydrate for electrolytic pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 513 MAGNESIUM 513 production of metal. Magnesium hydroxide produced from seawater alternatively may be calcined to magnesium oxide, MgO. The latter is reduced with carbon and converted to magnesium chloride by heating in an electric furnace in the presence of chlorine gas: electric MgO + C + Cl2 furnace → MgCl2 + CO electric MgO + CO + Cl2 furnace → MgCl2 + CO2 Manufacturing processes, based on thermal reduction of magnesium oxide employ ferrosilicon or carbon as a reducing agent and use dolomite as the starting material. In these processes, the mineral is first calcined to produce oxides of magnesium and calcium, MgO•CaO. In one such batch process, known as the Pidgeon process, calcined dolomite is mixed with pulverized ferrosilicon powder, briquetted, and charged into an electrically-heated retort made of nickel-chrome-steel alloy and operated under vacuum (0.1 to 0.2 mm Hg). The reaction is carried out at about 1,150°C for several hours (8 hours). Silicon reduces magnesium oxide to metallic magnesium produced as vapor. The vapors condense into crystals in the cooler zone of the retort (500°C). The reactions are as follows: 2(MgO•CaO) + Si(Fe) → 2 Mg + 2CaO•SiO2(Fe) The ferrosilicon alloy required in the above process is produced by thermal reduction of silica with carbon in the presence of iron: SiO2 + 2C + Fe → Si(Fe) + 2CO In the Pidgeon process discussed above, a secondary side reaction occurs between the CaO and SiO2 forming dicalcium silicate: 2CaO + SiO2 o C 1500 → Ca2SiO4 In a modified method known as Magnetherm process, sufficient aluminum oxide is added to melt this Ca2SiO4 slag. This allows the products to be removed in the molten state and, in addition, heats the reactor by the electrical resistance of the slag. Magnesium also is produced by thermal reduction of its oxide by carbon: MgO + C → Mg + CO The above reaction is reversible above 1,850°C. The metal produced as vapor must be cooled rapidly to prevent any reversible reactions. Rapid cooling (shock cooling) can quench the reaction giving finely divided pyrophoric dust pp-03-25-new dots.qxd 514 10/23/02 2:38 PM Page 514 MAGNESIUM of the metal. The separation, however, is difficult. This makes the carbon reduction process less attractive than the other two thermal reduction processes, namely Pidgeon and Magnetherm processes. Reactions At room temperature magnesium is not attacked by air. However, when heated it burns with a dazzling white light, forming the oxide, MgO and nitride, Mg3N2. The formation of oxide is an exothermic reaction. The heat of reaction causes a portion of the metal to combine with the nitrogen of air: 2Mg + O2 → 2 MgO 3Mg + N2 → 2 Mg3N2 When the metal is in a finely divided state or a thin foil, both the reactions above are rapid. Magnesium reacts very slowly with water at ordinary temperatures. Although the metal occupies a position higher than hydrogen in the electrochemical series, the reaction practically stops after a thin protective film of insoluble hydroxide deposits over the surface of the metal. The reaction is moderately fast in hot water and rapid in steam. The products are magnesium hydroxide and hydrogen: Mg + 2H2O → Mg(OH)2 + H2 In the presence of ammonium chloride or a substance that dissolves Mg(OH)2, the above reaction proceeds at ambient temperatures, the metal continues to dissolve in water, displacing hydrogen. Magnesium reacts readily with most mineral acids, evolving hydrogen: Mg + 2H+ → Mg2+ + H2 However, with certain acids, such as hydrofluoric acid, a protective layer of insoluble magnesium fluoride terminates the reaction. Likewise, the metal has little action on chromic acid. At ordinary temperatures magnesium is stable in alkalies, both dilute and concentrated. However, hot solutions of alkalies above 60°C attack the metal. Magnesium combines with halogens at elevated temperatures forming halides: Mg + Cl2 →MgCl2 Mg + Br2 →MgBr2 The metal reacts with nitrogen, phosphorus, sulfur and selenium at elevated temperatures forming their binary compounds: pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 515 MAGNESIUM 515 3Mg + N2 → Mg3N2 Mg + S →MgS 3Mg + 2P → Mg3P2 Magnesium exhibits single displacement reactions, thus replacing lower metals in electrochemical series from their salt solutions or melt. For example, magnesium will replace iron from molten iron(II) chloride forming magnesium chloride: Mg + FeCl2 → MgCl2 + Fe Or it will reduce Fe2+ to metallic iron from the aqueous solution of FeCl2: Mg + Fe2+ + 2Cl¯ → Mg2+ + 2Cl¯ + Fe Magnesium also reduces nonmetallic oxides, such as carbon dioxide, carbon monoxide, sulfur dioxide and nitrous oxide, burning at elevated temperatures. 2Mg + CO2 → 2MgO + C The metal reduces ammonia to magnesium nitride: 3Mg + 2NH3 → Mg3N2 + 3H2 Two important reduction reactions of magnesium that are of commercial interest are the production of titanium by Kroll process and obtaining uranium from its fluoride: 2Mg + TiCl4 → 2MgCl2 + Ti 2Mg + UF4 → 2MgF2 + U Magnesium forms hydride when heated with hydrogen under pressure: Mg + H2 → MgH2 Probably the most important reaction of magnesium in terms of synthetic applications involves preparation of Grignard reagent, RMgX where R is an alkyl or aryl group and X is a halogen other than fluorine. Grignard reagents provide convenient routes for various organic syntheses. These reagents are made by the reaction of magnesium with an alkly or aryl halide in ether: Mg + C2H5Br ether → C2H5MgBr (ethyl magnesium bromide) pp-03-25-new dots.qxd 516 10/23/02 2:38 PM Page 516 MAGNESIUM ACETATE Analysis Magnesium in trace amounts can be measured conveniently in aqueous and solid matrices by flame atomic absorption or by ICP emission spectroscopy. The sample is digested with nitric acid and diluted. The recommended wavelength for flame AA measurement is 285.2nm and for ICP/AES analysis 279.08 or 279.55 nm. The metal also can be measured by the gravimetric method in which diammonium hydrogen phosphate (NH4)2HPO4 is added to an ammoniacal solution of magnesium or its compound to produce a yellow precipitate of magnesium ammonium phosphate which on ignition yields magnesium pyrophosphate, Mg2P2O7. The solid or aqueous sample is digested with nitric acid and then hydrochloric acid, evaporated and diluted prior to adding (NH4)2HPO4 and ammonia solution. The method is less sensitive than the AA or ICP techniques and also subject to interference from calcium, aluminum, iron, silica and ammonium chloride. MAGNESIUM ACETATE [142-72-3] Formula: Mg(OOCCH3)2; MW 142.39; also exists as stable tetrahydrate, Mg(OOCCH3)2•4H2O [16674-78-5] and monohydrate Mg(OOCCH3)2•H2O [60582-92-5]. Uses Magnesium acetate is used in the manufacture of rayon fiber for cigarette filters; and as a fixative for dyes in textile printing. It also is used as an antiseptic and disinfectant. Physical Properties Anhydrous magnesium sulfate is a white crystalline solid occurring in alpha form as orthorhomic crystals or as a beta form having triclinic structure; density 1.507 and 1.502 g/cm3 for alpha- and beta-forms, respectively; decomposes at 323°C; very soluble in water; moderately soluble in methanol (5.25g/100 mL at 15°C). The tetrahydrate constitutes colorless monoclinic crystals; hygroscopic; density 1.454 g/cm3; melts at 80°C; highly soluble in water (120 g/100mL at 15°C); very soluble in methanol and ethanol. Preparation Magnesium acetate is prepared by treating magnesium oxide with acetic acid. Magnesium oxide reacts with concentrated acetic acid in boiling ethyl acetate to produce the alpha form of anhydrous magnesium acetate. The beta form is obtained by treating the oxide with 5–6% acetic acid. In slightly hydrated isobutyl alcohol medium the product is a monohydrate, Mg(OOCCH3)2•H2O. In aqueous solution magnesium acetate crystallizes as a tetrahydrate, the commercial product. The tetrahydrate dehydrates to anhy- pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 517 MAGNESIUM BROMIDE 517 drous salt at 134°C. Analysis Elemental composition for anhydrous acetate: Mg 17.08%, C 33.73%, H 4.25%, O 44.74%. The water of crystallization in the commercial product can be measured by gravimetry. Acetate anion can be estimated from elemental analysis for C, H and O, or by ion chromatography in a very dilute aqueous solution. Mg can be determined by AA or ICP methods. MAGNESIUM BROMIDE [7789-48-2] Formula: MgBr2; MW 184.11; forms stable hexahydrate, MgBr2•6H2O [13446-53-2] and decahydrate, MgBr210H2O [75198-45-7]. Occurrence and Uses Magnesium bromide occurs in sea water, surface and subterranean brines, and salt deposits. It is an electrolyte component in certain dry cells. In medicine, it is a sedative and anticonvulsant for treatment of nervous disorder. It also is used in organic synthesis forming several addition compounds. Physical Properties The anhydrous MgBr2 is a white crystalline substance; hexagonal crystals; deliquescent; density 3.72 g/cm3; melts at 700°C; highly soluble in water (101.5g/100mL at 20°C); moderately soluble in methanol and ethanol (21.8 and 6.9 g/mL at 20°C, respectively). The hexahydrate, MgBr2•6H2O consists of colorless monoclinic crystals; bitter taste; hygroscopic; fluoresce in x-rays; density 2.07 g/cm3; melts at 172.4°C; intensely soluble in water, 316 g/100 mL at 0°C; dissolves in methanol and ethanol; slightly soluble in ammonia solution. Thermochemical Properties ∆Hƒ° (cry) ∆Hƒ° (gas) ∆Hƒ° (aq) ∆Gƒ° (cry) S° (cry) –125.3 kcal/mol –74.0 kcal/mol –169.7 kcal/mol –120.4 kcal/mol 28.0 cal/degree mol Preparation Magnesium bromide is prepared by treating magnesium oxide with hydrobromic acid and subsequent crystallization above 0°C. The product is hexahydrate, MgBr2•6H2O: MgO + 2HBr → MgBr2 + H2O The anhydrous MgBr2 may be obtained by heating the hexahydrate with pp-03-25-new dots.qxd 518 10/23/02 2:38 PM Page 518 MAGNESIUM CARBONATE dry hydrogen bromide gas. Magnesium bromide also can be made from its elements. Heating magnesium metal with bromine vapor yields the salt: Mg + Br2 → MgBr2 Magnesium bromide, like the chloride salt, is obtained from sea water (see Magnesium and Magnesium chloride). In this process, magnesium hydroxide precipitated from sea water is neutralized with hydrobromic acid, and MgBr2 is obtained by crystallization. Analysis Elemental composition: Mg 13.20%, Br 86.80%. The aqueous solution is analyzed for Mg by AA or ICP technique and the bromide ion measured by ion chromatography. MAGNESIUM CARBONATE [13717-00-5] Formula: MgCO3; MW 84.31; several hydrated and basic carbonates are also known that are stable and occur in nature. The types, names, formulas and CAS Registry numbers of anhydrous, hydrated and basic magnesium carbonates are tabulated below: Compound Mineral anhydrous salt dihydrate trihydrate pentahydrate basic carbonate basic carbonate basic carbonate basic carbonate magnesite MgCO3 barringtonite MgCO3•2H2O nesquehonite MgCO3•3H2O lansfordite MgCO3•5H2O artinite MgCO3•Mg(OH)2•3H2O hydromagnestite 4MgCO3•Mg(OH)2•4H2O dypingite 4MgCO3•Mg(OH)2•5H2O __ 4MgCO3•Mg(OH)2•8H2O Formula CAS No. [13717-00-5] [5145-48-2] [14457-83-1] [61042-72-6] [12143-96-3] [12072-90-1] [12544-02-4] [75300-49-1] Occurrence and Uses Magnesium carbonate occurs in nature in several minerals as hydrated, basic and double salts, as shown above. The two principal minerals are magnesite, MgCO3 and dolomite, a double salt, CaCO3•MgCO3. Both minerals are used as source materials in the production of magnesium metal. Also, they are calcined to produce basic refractory bricks. Other applications of magnesium carbonate are in flooring, fireproofing and fire-extinguishing compositions; as a filler material and smoke suppressant in plastics; as a reinforcing agent in neoprene rubber; as a drying agent and for color retention in foods; in cos- pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 519 MAGNESIUM CARBONATE 519 metics; in dusting powder; and in toothpaste. The high purity magnesium carbonate is used as an antacid in medicine; and as an additive to table salt. Another important application of magnesium carbonate is as a starting material in producing a number of magnesium compounds. Physical Properties The anhydrous salt consists of white trigonal crystals; refractive index 1.717; density 2.958 g/cm3; decomposes at 350°C; practically insoluble in water (106 mg/L at room temperature); Ksp 1.0x10–5; low to moderate solubility under partial pressure of CO2 (3.5 and 5.9 g MgCO3/100g saturated solution at CO2 pressure 2 and 10 atm, respectively); insoluble in acetone and ammonia; dissolves in acids. The di– and trihydrates, MgCO3•2H2O and MgCO3•3H2O are colorless crystals having triclinic and monoclinic structures, respectively; the refractive index 1.458 and 1.412, respectively; and their densities are 2.825 and 1.837 g/cm3. The pentahydrate, MgCO3•5H2O, occurring naturally as the mineral lansfordite is a white crystalline solid; monoclinic crystals; refractive index 1.456; density 1.73g/cm3; decomposes in air; slightly soluble in water (0.375 g/100 mL at 20°C). All three basic carbonates, artinite, hydromagnestite and dypingite, are white crystalline substances of monoclinic crystal structures; refractive index 1.488, 1.523 and 1.508, respectively; the index of refraction for the basic carbonate octahydrate is 1.515; the densities are 2.02 and 2.16 g/cm3 for artinite and hydromagensite; the basic carbonates are all practically insoluble in water. Thermochemical Properties ∆Hƒ° (MgCO3) ∆Gƒ° (MgCO3) ∆Gƒ° (MgCO3•3H2O) ∆Gƒ° (MgCO3•5H2O) S° (MgCO3) Cρ (MgCO3) –261.9 kcal/mol –241.9 kcal/mol –412.6 kcal/mol –525.7 kcal/mol 15.7 cal/degree mol 18.05 cal/degree mol Preparation Magnesium carbonate is obtained mainly by mining its natural mineral magnesite. The trihydrate salt, MgCO3•3H2O, is prepared by mixing solutions of magnesium and carbonate ions in the presence of carbon dioxide. Alternatively, it may be produced by carbonation of a magnesium hydroxide slurry with carbon dioxide under pressure (3.5 to 5 atm) and at a temperature below 50°C which yields soluble magnesium bicarbonate: Mg(OH)2 + 2CO2 → Mg(HCO3)2 The solution is filtered to remove impurities and the filtrate is subjected to vacuum or aeration to yield insoluble magnesium carbonate as a hydrated salt: pp-03-25-new dots.qxd 520 10/23/02 2:38 PM Page 520 MAGNESIUM CARBONATE Mg2 + 2HCO3¯ → MgCO3 + CO2 + H2O Under ordinary conditions, anhydrous magnesium carbonate cannot be prepared in aqueous systems. The anhydrous salt, however, can be made under very high partial pressures of carbon dioxide. Basic magnesium carbonate occurs in nature as the mineral hydromagnesite. The basic salt is obtained by mining the ore followed by purification. The basic carbonates also can be made by drying the magnesium carbonate trihydrate at about 100°C. Alternatively it can be prepared by simply boiling a solution of magnesium bicarbonate. The bicarbonate is obtained by carbonation of a magnesium hydroxide slurry below 50°C and under a CO2 partial pressure of 3.5 to 5 atm. Composition of the basic carbonate produced by the above methods is 4MgCO3 •Mg(OH)2•4H2O. Another basic salt, MgCO3•Mg(OH)3•3H2O is precipitated when magnesium salt solution is treated with sodium carbonate solution. The reactions probably are: CO32– + H2O → HCO3¯ + OH¯ 2Mg2+ + CO32– + 2OH¯ → MgCO3•Mg(OH)2 Reactions Magnesium carbonate dissolves in dilute mineral acids, evolving carbon dioxide: MgCO3 + HCl → MgCl2 + CO2 + H2O MgCO3 + H2 SO4 → MgSO4 + CO2 + H2O Thermal dissociation at elevated temperatures yields magnesium oxide and CO2: MgCO3 → MgO + CO2 The trihydrate, MgCO3•3H2O or other hydrates on heating form basic magnesium carbonates, the product compositions depending on degree of water of crystallization and temperature. Magnesium carbonate forms several double salts with salts of alkali and alkaline earth metals and ammonium ion. Some examples are: MgCO3•Na2CO3; MgCO3•K2CO3•8H2O; MgCO3•KHCO3•4H2O (Engle’s salt); MgCO3•(NH4)2CO3•4H2O; MgCO3•MgCl2•7H2O, and MgCO3•MgBr2•7H2O Analysis Elemental composition: Mg28.83%, C 14.24%, O 56.93%. A measured pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 521 MAGNESIUM CHLORIDE 521 amount of magnesium carbonate is treated with dilute HCl and liberated CO2 is identified by the limewater test (CO2 turns limewater milky). Carbon dioxide also may be identified and quantified by GC-TCD or preferably by GC/MS (characteristic mass ion 44). The acid solution can be analyzed for magnesium by AA or ICP techniques. MAGNESIUM CHLORIDE [7786-30-3] Formula: MgCl2; MW 95.218; also occurs as hexahydrate, MgCl2•6H2O [13778-96-6]. Occurrence and Uses Magnesium chloride is a constituent of sea water. It also is found in most natural brines and many minerals such as carnallite, KCl•MgCl2•H2O. Its hexahydrate occurs in nature as mineral bischofite, MgCl2•6H2O. The most important use of magnesium chloride is in the electrolytic production of magnesium metal. The compound is also used to make oxychloride cement, or what is known as Sorel cement for flooring, fire-resistant panel, and fireproofing of steel beams and other materials. Other applications are: as a dust binder on roads; as a flocculating agent in water treatment; for dressing cotton and woolen fabrics; as a fire-extinguishing agent and a fireproofing material; in processing of sugar-beets; and as a catalyst. Physical Properties Anhydrous salt consists of white lustrous hexagonal crystals; refractive index 1.675; density 2.32 g/cm3; melts at 714°C; decomposes at a lower temperature of 300°C when heated slowly, releasing chlorine; vaporizes at 1,412°C; highly soluble in water, releasing heat (solubility 54.2 g/100 mL at 20°C and 72.7 g/100mL at 100°C) moderately soluble in ethanol (7.4 g/100mL at 30°C). Hexahydrate constitutes colorless monoclinic crystals; deliquescent; refractive index 1.495; density 1.569 g/cm3; decomposes on heating at 116°C; highly soluble in water (157 g/100mL at 20°C); solubility increased on heating; soluble in alcohol. Thermochemical Properties ∆Hƒ° (MgCl2) ∆Hƒ° (MgCl2•6H2O) ∆Gƒ° (MgCl2) ∆Gƒ° (MgCl2•6H2O) S° (MgCl2) S° (MgCl2•6H2O) Cρ (MgCl2) Cρ (MgCl2•6H2O) –153.28 kcal/mol –597.28 kcal/mol –141.45 kcal/mol –505.49 kcal/mol 21.42 cal/degree mol 87.50 cal/degree mol 17.06 cal/degree mol 75.30 cal/degree mol pp-03-25-new dots.qxd 522 10/23/02 2:38 PM Page 522 MAGNESIUM CHLORIDE Production Magnesium chloride is prepared by treating magnesium carbonate, hydroxide or oxide with hydrochloric acid followed by crystallization by evaporation. The hexahydrate of the salt MgCl2•6H2O is obtained upon crystallization. In most commercial processes, the compound is either derived from the sea water or from the natural brines, both of which are rich sources of magnesium chloride. In the sea water process, the water is treated with lime or calcined dolomite (dolime), CaO•MgO or caustic soda to precipitate magnesium hydroxide. The latter is then neutralized with hydrochloric acid. Excess calcium is separated by treatment with sulfuric acid to yield insoluble calcium sulfate. When produced from underground brine, brine is first filtered to remove insoluble materials. The filtrate is then partially evaporated by solar radiation to enhance the concentration of MgCl2. Sodium chloride and other salts in the brine concentrate are removed by fractional crystallization. The crude product containing magnesium oxide or hydroxide is purified by heating with chlorine. Magnesium chloride can be also recovered from its mineral carnallite by similar processes involving concentration of the liquor by solar evaporation followed by separation of other salts by fractional crystallization. The product obtained is always the hexahydrate, MgCl2•6H2O. It is dehydrated to anhydrous magnesium chloride by spray drying and heating with dry hydrogen chloride gas. In the absence of HCl, heating hexahydrate yields the basic salt, Mg(OH)Cl: MgCl2•6H2O → Mg(OH)Cl + HCl + 5H2O Pure anhydrous chloride can be prepared by heating the double salt MgCl2•NH4Cl•6H2O: MgCl2•NH4Cl•6H2O → MgCl2•NH4Cl + 6H2O Ammonium chloride sublimes on further heating, leaving pure anhydrous MgCl2: MgCl2•NH4Cl → MgCl2 + NH4Cl Other methods of preparation involve heating magnesium oxide with coke powder in the presence of chlorine: MgO + C + Cl2 → MgCl2 + CO Magnesium chloride also is a by-product during reduction of titanium(IV) chloride with magnesium metal: TiCl4 + 2Mg → Ti + 2MgCl2 The anhydrous salt and the hexahydrate are both highly corrosive. They are handled in equipment made out of inconel. pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 523 MAGNESIUM FLUORIDE 523 Analysis Elemental composition (anhydrous MgCl2): Mg 25.54%, Cl 74.46%. Aqueous solution of the salt may be analyzed for Mg by AA or ICP method (See Magnesium). The chloride ion can be identified by ion chromatography or measured by titration with a standard solution of silver nitrate using potassium chromate as indicator. MAGNESIUM FLUORIDE [7783-40-6] Formula: MgF2; MW 62.31 Synonym: magnesium flux Occurrence and Uses Magnesium fluoride occurs in nature as the mineral, sellaite. It is used in glass and ceramics. Single crystals are used for polarizing prisms and lenses. Physical Properties Colorless tetragonal crystals; faint violet luminescence; refractive index 1.378; density 3.148 g/cm3; Moh’s hardness 6; melts at 1261°C; vaporizes at 2,260°C; practically insoluble in water (76 mg/L at 18°C); soluble in nitric acid; slightly soluble in dilute acids and acetone; insoluble in ethanol. Thermochemical Properties ∆Hƒ° ∆Gƒ° S° Cρ –268.5 kcal/mol –255.8 kcal/mol 13.68 cal/degree mol 14.72 cal/degree mol Preparation Magnesium fluoride is prepared by treating a magnesium salt solution with hydrofluoric acid or sodium fluoride: MgSO4 + 2HF → MgF2 + 2H+ + SO42– or by adding hydrofluoric acid to magnesium carbonate: MgCO3 + 2HF → MgF2 + CO2 + H2O Analysis Elemental composition: Mg 39.02%, F 60.98%. The compound is digested with nitric acid-hydrofluoric acid mixture, diluted and analyzed for magnesium by AA or ICP method. The crystals may be characterized nondestructively by x-ray crystallography. pp-03-25-new dots.qxd 524 10/23/02 2:38 PM Page 524 MAGNESIUM HYDRIDE MAGNESIUM HYDRIDE [60616-74-2] Formula: MgH2; MW 26.321 Uses Magnesium hydride is a reducing agent; a source of hydrogen; and serves to prepare many complex hydrides. Physical Properties White tetragonal crystals; rutile structure; density 1.45 g/cm3; decomposes at 200°C; reacts with water. Preparation Magnesium hydride is obtained by combining the elements at about 500°C. A convenient method of preparation involves passing hydrogen under pressure over heated magnesium powder in the presence of magnesium iodide as catalyst. high temperature Mg + H2 and pressure −−−−−−−−→ MgH2 Mgl 2 Magnesium hydride also is produced by thermal decomposition of diethylmagnesium at 200°C: (C2H5)2Mg → MgH2 + C4H8 An active form of the hydride obtained as a solvated pyrophoric powder and used as a reducing agent is prepared by the reaction of dibutylmagnesium (C4H9)2Mg with phenylsilane, C6H5SiH3 in ether-heptane solvent mixture. Reactions Magnesium hydride is not readily decomposed by heat. However, in high vacuum decomposition takes place at 280°C, the hydride dissociating to its elements. Magnesium hydride is a strong reducing agent, reducing oxidizable substances and compounds containing oxygen. The reactions often progress with violence. It ignites spontaneously in air, forming magnesium oxide and water: MgH2 + O2 → MgO + H2O It reacts violently with water, evolving hydrogen. Similar reaction occurs with methane forming magnesium methoxide and evolving hydrogen: MgH2 + 2CH3OH → Mg(OCH3)2 + 2H2 pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 525 MAGNESIUM HYDROXIDE 525 Magnesium hydride forms double hydrides with aluminum hydride and boron hydride: MgH2 + B2H6 ether → MgB2H8 MgH2 + 2AlH3 ether → MgAl2H8 Analysis Elemental composition: Mg 92.35%, H 7.65%. The compound may be identified from its chemical properties that involve the evolution of hydrogen when cautiously treated with water or methanol (See Hydrogen). Magnesium may be analyzed by various instrumental techniques after digesting the compound into aqueous phase aided by nitric acid. Hazard Flammable solid, ignites spontaneously in air. Reaction with water is violent with the evolution of hydrogen. MAGNESIUM HYDROXIDE [1309-42-8] Formula: Mg(OH)2; MW 58.327 Synonym: brucite Occurrence and Uses Magnesium hydroxide occurs in nature as mineral brucite, often associated with several other minerals such as calcite, magnesite, or talc. Magnesium hydroxide is used as an intermediate in making magnesium metal. It also is used to manufacture magnesium oxide, magnesium carbonate and several other magnesium salts. Milk of magnesia, a finely divided suspension of magnesium hydroxide in water, is used in medicine as a laxative and antacid. Physical Properties Colorless hexagonal plate; refractive index 1.559; density 2.36 g/cm3; loses water at 350°C; practically insoluble in water (9mg/L at 18°C and 40 mg/L at 100°C); soluble in acids and in aqueous solutions containing NH4+ ion. Thermochemical Properties ∆Hƒ° ∆Gƒ° S° Cρ –220.97 kcal/mol –199.23 kcal/mol 15.10 cal/degree mol 18.41 cal/degree mol pp-03-25-new dots.qxd 526 10/23/02 2:38 PM Page 526 MAGNESIUM HYDROXIDE Production Magnesium hydroxide is commonly produced from seawater, which is rich in Mg2+ ion. The average concentration of Mg2+ in seawater is about 1,300 mg/L. The first step of the process involves removal of interfering substances from seawater, the most notable being the water-soluble calcium bicarbonate. Bicarbonate removal is crucial, as it can form insoluble calcium carbonate, a side product that cannot be separated from magnesium hydroxide readily. Acidification of seawater converts bicarbonate into carbon dioxide, which is degassed by heating. Alternatively, seawater is treated with lime to convert calcium bicarbonate to carbonate: Ca(HCO3)2 + CaO → 2CaCO3 + H2O Lime is obtained by calcination of dolomite, CaCO3•MgCO3, or limestone, CaCO3, under controlled conditions to remove all CO2. After bicarbonate removal, the seawater is then treated with calcium hydroxide, slaked dolime or sodium hydroxide to precipitate magnesium hydroxide: Mg2+ + 2OH¯ → Mg(OH)2 The solution is seeded with magnesium hydroxide to enhance crystal growth. Magnesium hydroxide also is obtained from waste liquors from the potash industry. It is precipitated from mother liquors containing magnesium salts. In the laboratory, magnesium hydroxide may be prepared by double decomposition reactions by adding a soluble hydroxide to solutions of magnesium salts; i.e., adding caustic soda solution to magnesium sulfate solution: Mg2+ + SO42– + 2Na+ + 2OH¯ → Mg(OH)2 + 2Na+ + SO42– The above precipitation reaction does not occur with ammonium hydroxide in the presence of excess ammonium chloride. Reactions Solid magnesium hydroxide is decomposed by heat, forming magnesium oxide: Mg(OH)2 → MgO + H2O Magnesium hydroxide is a weak base. However, it is sufficiently strong to neutralize acids, forming their salts. For example, treatment with sulfuric acid followed by evaporation and crystallization yields magnesium sulfate: Mg(OH)2 + H2SO4 → MgSO4 + 2H2O Magnesium hydroxide is soluble in solutions containing excess ammonium ion: Mg(OH)2 + 2NH4+ → Mg2+ + 2NH4OH pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 527 MAGNESIUM IODIDE 527 Carbonation of its slurry with carbon dioxide at 4 to 5 atm pressure yields magnesium bicarbonate: Mg(OH)2 + CO2 → Mg(HCO3)2 Treatment with sodium carbonate solution yields basic carbonate. The probable reaction step is as follows: 2Mg2+ + 2OH¯ + CO32– → MgCO3•Mg(OH)2 Similarly, basic magnesium chloride of indefinite composition is produced when magnesium hydroxide is mixed with magnesium chloride and water. The product is used as oxychloride cement (see Magnesium Oxide). MAGNESIUM IODIDE [10377-58-9] Formula: MgI2; MW 278.12; forms two stable hydrates, hexahydrate MgI2•6H2O [75535-11-4] and octahydrate MgI2•8H2O [7790-31-0]. Uses Magnesium iodide has few commercial applications. The salt is used to prepare several addition compounds with organic solvents, some of which are used in organic synthesis. Physical Properties The anhydrous iodide is white hexagonal solid; deliquescent; density 4.43 g/cm3; decomposes at 637°C; highly soluble in water (148 g/100mL at 18°C); soluble in alcohol, ether and ammonia. The octahydrate is white orthorhombic crystals; deliquescent; density 2.098 g/cm3; decomposes at 41°C; very soluble in water (81g/100 mL at 20°C); soluble in alcohol and ether. Thermochemical Properties ∆Hƒ° ∆Gƒ° S° –87.0 kcal/mol –85.6 kcal/mol 31.0 cal/degree mol Preparation Magnesium iodide is prepared by the reaction of magnesium oxide, hydroxide or carbonate with hydriodic acid, followed by evaporation of the solution and crystallization: MgO + 2HI → MgI2 + H2O pp-03-25-new dots.qxd 528 10/23/02 2:38 PM Page 528 MAGNESIUM NITRATE Mg(OH)2 + 2HI → MgI2 + 2H2O MgCO3 + 2HI → MgI2 + CO2 + H2O Analysis Elemental composition (anhydrous MgI2): Mg 8.72%, I 91.26%. Aqueous solution may be analyzed for Mg by AA or ICP, and for iodide by ion chromatography following appropriate dilution. MAGNESIUM NITRATE [10377-60-3] Formula: Mg(NO3)2; MW 148.31; forms two stable hydrates; the hexahydrate Mg(NO3)2•6H2O [13446-18-9] and the dihydrate, Mg(NO3)2•2H2O [15750-45-5]. Occurrence and Uses The hexahydrate, Mg(NO3)2•6H2O, occurs in nature as mineral nitromagnesite. Magnesium nitrate is used in pyrotechnics; and in the manufacture of concentrated nitric acid to remove water and concentrate the acid vapors to 90–95% HNO3. It also is used to aid coating and prilling in production of ammonium nitrate. The salt also is used as an analytical standard for magnesium and a matrix modifier in furnace atomic absorption spectroscopic analysis. It also finds some limited application as a nitrogenous fertilizer. Physical Properties The anhydrous salt consists of white cubic crystals; density 2.3 g/cm3; very soluble in water. The dihydrate is white crystalline solid having density 1.45 g/cm3; decomposes at about 100°C; soluble in water and ethanol. The hexahydrate, MgNO3•6H2O is a colorless solid having monoclinic crystal structure and density 1.46 g/cm3. The salt is hygroscopic and very soluble in water and moderately soluble in ethanol. Thermochemical Properties ∆Hƒ° ∆Gƒ° S° Cρ –189.0 kcal/mol –147.4 kcal/mol 39.2 cal/degree mol 33.9 cal/degree mol Preparation Magnesium nitrate is prepared by the action of nitric acid on magnesium carbonate, oxide or hydroxide: MgCO3 + 2HNO3 → Mg(NO3)2 + CO2 + H2O pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 529 MAGNESIUM OXIDE 529 Mg(OH)2 + 2HNO3 → Mg(NO3)2 + 2H2O The salt crystallizing at room temperature after evaporation is the hexahydrate, Mg(NO3)2•2H2O. Reactions Thermal decomposition of anhydrous Mg(NO3)2 yields magnesium oxide and nitrogen oxides. Heating the hexahydrate above its melting point forms basic nitrates, such as Mg(NO3)2•4 Mg(OH)2. The latter decomposes at 400°C, forming magnesium oxide and oxides of nitrogen. Magnesium nitrate forms addition compounds with a number of nitrogen-containing organics such as pyridine, aniline, and urea. Analysis Elemental composition (anhydrous Mg(NO3)2); Mg 16.39%, N 18.88%, O 64.73%. The water of crystallization can be measured by gravimetry. Magnesium content of the salt can be measured by analysis of the metal in an aqueous solution using AA or ICP. Nitrate anion can be measured by ion chromatography—or by using a nitrate ion-selective electrode. MAGNESIUM OXIDE [1309-48-4] Formula: MgO; MW 40.30 Synonym: magnesia; magnesia usta Uses Magnesium oxide occurs in nature as the mineral periclase. The commercial product is manufactured in several grades, depending on the purity, particle size and the reactivity desired. Dead-burned magnesia (consisting of sintered micro-crystals) is used in production of basic refractory brick for cement kilns, furnaces and crucibles. The caustic-burned magnesia, more reactive than the dead-burned reactive grade, is used to manufacture various magnesium salts; in extraction of uranium oxide from uranium ore; as mineral supplement in animal feed; and in many catalytic applications. Caustic-burned magnesia of higher reactive-grade, available as light or heavy magnesia, is used in cosmetics as fillers; as an accelerator for vulcanization of rubber; as an ingredient of antacids; and to prepare magnesium metal and various metal salts. Fused magnesia in crushed form is used in electrical arc furnaces and domestic appliances as insulation. Physical Properties Periclase: Colorless, transparent cubic crystals or white very-fine powder; refractive index 1.736; density 3.58 g/cm3; hardness 5.5 Mohs; melts at pp-03-25-new dots.qxd 530 10/23/02 2:38 PM Page 530 MAGNESIUM OXIDE 2,852°C; vaporizes at 3,600°C; electrical resistivity 1.3x1015 ohm–cm at 27°C; practically insoluble in water (86 mg/L at 30°C); soluble in acids and ammonium salt solutions; insoluble in alcohol. Thermochemical Properties ∆Hƒ° ∆Gƒ° S° Cρ Thermal conductivity at 27°C –143.81 kcal/mol –136.10 kcal/mol 6.44 cal/degree mol 8.88 cal/degree mol 60.0 W/m.K Production Magnesium oxide is produced either from its minerals or from seawater or brine. Among minerals, magnesite, MgCO3 and dolomite, MgCO3•CaCO3 are the two primary sources. It also may be obtained from its hydroxide ore, brucite, Mg(OH)2. Calcination of these minerals yields magnesium oxide. The minerals generally contain several impurities, such as silica, alumina, iron oxide, and oxides and silicates of calcium and other metals. The ore is crushed, sized and impurities are separated by various processes, including froth flotation, magnetic separation, dissolution, and a wide-range of chemical process depending on the chemical properties of impurities. Often magnesium ore is converted into one of its salts, such as carbonate, hydroxide, chloride, or sulfate by chemical processes. The salt on calcination yields magnesium oxide: MgCO3 calcinatio n → MgO + CO2 Mg(OH)2 calcinatio n → MgO + H2O If dolomite is the source, thermal decomposition of MgCO3 at 350°C produces MgO. At this temperature, CaCO3 does not decompose. The decomposition temperature for the latter is 850°C. Magnesium oxide also is produced from sea water and subterranean brine. Magnesium ion is precipitated as hydroxide by treating seawater with calcium or sodium hydroxide following a series of concentration steps (See magnesium). The hydroxide is then calcined to yield oxide. If brine is the source, it is concentrated, purified and calcined: MgCl2 + H2O → MgO + 2HCl Calcination temperature is very important in the production process and dictates the particle size, purity and reactivity of the product. A dead-burned, sintered dense microcrystalline product is obtained at calcination temperature of 1,400 to 1,700°C. A caustic-burned product is obtained when magnesium carbonate or hydroxide is calcined at 600 to 700°C. A light grade (specific gravity 2.9) highly reactive caustic-burned magnesia that contains some moisture and carbon dioxide is obtained at about 600°C. A denser form from pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 531 MAGNESIUM PERCHLORATE 531 heavy caustic-burned oxide is produced when the carbonate or hydroxide is calcined at 800 to 900°C. Magnesium oxide also can be prepared by heating magnesium metal in oxygen. Reactions Unlike calcium oxide, at ordinary temperatures magnesium oxide is stable in water. There is very little formation of magnesium hydroxide. The reaction, however, is rapid at elevated temperatures. The acids form their magnesium salts which, if water-soluble, may be obtained by evaporation of the solution: MgO + H2SO4 → MgSO4 + H2O MgO + 2HCl → MgCl2 + H2O Heating the oxide with carbon dioxide yields magnesium carbonate, MgCO3. The oxide can be reduced to metallic magnesium by heating with a reducing agent such as carbon or hydrogen at elevated temperatures: MgO + C → Mg + CO MgO + H2 → Mg + H2O Analysis Elemental composition: Mg 60.32%, O 39.68%. The oxide can be identified nondestructively by x-ray methods. Oxygen content may be determined by elemental microanalysis. Magnesium may be analyzed by AA or ICP following dissolution of the oxide in nitric acid and appropriate dilution with water. MAGNESIUM PERCHLORATE [10034-81-8] Formula: Mg(ClO4)2; MW 223.21; forms several hydrates including a stable hexahydrate, Mg(ClO4)2•6H2O Synonyms: Anhydrone; Dehydrite Uses Magnesium perchlorate is a drying agent for gases; and also an oxidizing agent. Physical Properties White granular or flaky powder; highly deliquescent; density 2.21 g/cm3; decomposes at 251°C; very soluble in water (99.3g/100mL at 18°C); soluble in ethanol (24g/100mL) at 25°C. Hexahydrate constitutes white rhombohedral crystals; refractive index pp-03-25-new dots.qxd 532 10/23/02 2:38 PM Page 532 MAGNESIUM PHOSPHATES, BASIC 1.482; density 1.98 g/cm3; melts around 185°C; very soluble in water, releasing heat. Preparation Magnesium perchlorate may be prepared by adding perchloric acid to an aqueous solution of magnesium hydroxide. Crystallization yields hexahydrate, Mg(ClO4)2•6H2O. Mg(OH)2 + 2HClO4 → Mg(ClO4)2 + H2O Reactions Magnesium perchlorate is a strong oxidizing agent. In aqueous solutions and in acid medium the most conspicuous reactions are those involving oxidation—characteristic of the oxidizing action of perchlorate ion, ClO4¯. Thermal decomposition in the presence of a catalyst, such as manganese dioxide, yields magnesium chloride and oxygen: Mg (ClO4)2 heat −−−−−−−−→ MgCl2 + 4O2 catalyst Analysis Elemental composition (for anhydrous salt): Mg 10.89%, Cl 31.77%, O 57.34%. In the aqueous solution of the compound, Mg is analyzed by AA or ICP and perchlorate ion by ion chromatography or by redox titration. Also the solid salt may be mixed with MnO2 and heated. Oxygen liberated may be tested by flaming of a glowing splinter, and the MgCl2 residue may be dissolved in water, filtered, and the aqueous solution may be analyzed for Cl¯ by titration or ion chromatography and Mg determined by AA or ICP (See Magnesium Chloride). MAGNESIUM PHOSPHATES, BASIC Magnesium phosphate forms three basic salts, as follows: (i) Monobasic salt: MgH4(PO4)2; MW 218.28; CAS No. [13092-66-5] Synonyms: magnesium biphosphate; primary magnesium phosphate; acid magnesium phosphate; magnesium tetrahydrogen phosphate (ii) Dibasic salt: MgHPO4; MW 120.29; CAS No. [7757-86-0]; also forms a stable trihydrate, MgHPO4•3H2O; the trihdrate is found in nature as the minerals, newberyite and phosphorroeslerite. Synonyms: magnesium hydrogen phosphate; secondary magnesium phosphate (iii) Tribasic salt: Mg3(PO4)2; MW 262.86; CAS No. [7757-87-1]; forms stable hydrates Mg3(PO4)2•4H2O, Mg3(PO4)2•8H2O, and Mg3(PO4)2•22H2O; the octahydrate occurs naturally as the mineral bobierrite. Synonyms: magnesium orthophosphate, neutral magnesium phosphate, tri- pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 533 MAGNESIUM PHOSPHATES, BASIC 533 magnesium phosphate Uses All basic magnesium phosphates find applications in plastics as stabilizers. Other than this, monobasic salt is used in fireproofing wood. The dibasic phosphate is a food additive; and also a laxative. The tribasic phosphate is an antacid; and a nutritional food supplement. The compound also is an adsorbent; and a polishing agent in dental work. Physical Properties The monobasic phosphate as dihydrate is a white crystalline powdery material; hygroscopic; decomposes on heating; dissolves in water; soluble in acids with reaction; insoluble in alcohol. The dibasic magnesium phospate trihydrate is a white crystalline powder; orthorhombic structure; refractive index 1.514; density 2.123 g/cm3 at 15°C; melts at 205°C losing a molecule of water; decomposes between 550 to 650°C; slightly soluble in water; soluble in acid; insoluble in ethanol. The heptahydrate MgHPO4•7H2O constitutes white monoclinic needles; density 1.728 g/cm3 at 15°C; sparingly soluble in water (3g/L at 20°C); soluble in acids; insoluble in ethanol. The tetrahydrate of the tribasic phosphate, Mg3(PO4)2•4H2O is a bulky and soft white powdery material; monoclinic crystals; density 1.64 g/cm3 at 15°C; slightly soluble in water (0.2 g/L at 20°C); soluble in acids. The naturally occurring octahydrate, bobierite, is a white crystalline solid, containing monoclinic plates; refractive index 1.510; density 2.195 g/cm3 at 15°C; loses three molecules of water of crystallization at 150°C; loses all water at 400°C; insoluble in water; soluble in dilute mineral acids. Magnesium orthophosphate Mg3(PO4)2 constitutes rhombic crystals; melts at 1,184°C; insoluble in water; soluble in ammonium salt solution. Thermochemical Properties [Mg3(PO4)2] ∆Hƒ° –903.6 kcal/mol ∆Gƒ° –845.8 kcal/mol S° 45.2 cal/degree mol Cρ 51.0 cal/degree mol Preparation The basic phosphates that occur naturally may be mined from their respective minerals. They may be prepared by reactions of phosphoric acid with magnesium oxide and hydroxide followed by crystallization. Monobasic and dibasic magnesium phosphate are prepared by the action of phosphoric acid on magnesium hydroxide and magnesium oxide, respectively. The tribasic phosphate is made by treating magnesium oxide with phosphoric acid at high temperature. Analysis Basic magnesium phosphates may be characterized by x-ray and thermogravimetric analyses and elemental analysis. Magnesium may be determined pp-03-25-new dots.qxd 534 10/23/02 2:38 PM Page 534 MAGNESIUM SILICATES by AA or ICP after digestion in nitric acid followed by dilution. Alternatively, the compounds can be analyzed for magnesium nondestructively, but with lesser sensitivity, using x-ray fluorescence. The phosphorus content may be measured by dissolving the basic phosphate in sulfuric acid, diluting the acid extract and treating the diluted acid solution with ammonium molybdateammonium metavanadate reagent, and measuring the intensity of the yellow color formed using a spectrophotometer at 400 to 490 nm wavelength. Alternatively, the acid solution may be treated with ammonium molybdate and stannous chloride reagent to produce an intense blue color that may be measured at 690 or 650 nm. The concentration may be determined from a phosphate standard calibration curve (APHA, AWWA, and WEF. 1999. Standard Methods for the Examination of Water and Wastewater, 20th ed. Washington D.C.: American Public Health Association.) MAGNESIUM SILICATES Magnesium forms an array of silicates having varying structures. Such a wide variety of silicates include metasilicate, orthosilicate, pyrosilicate, polysilicates, and a number of complex silicates, such as asbestos and talc in combination with other metal ions. Many such silicates occur in nature either as complex silicates or as discrete magnesium silicate. Some important magnesium silicates are listed below: (i) Magnesium metasilicate: MgSiO3 [13776-74-4]; MW 100.39; occurs in nature as minerals enstatite, clinoenstatite, and protoenstatite. It has pyroxene-type structure consisting of (SiO32–)n chain. The metasilicate consists of white monoclinic crystals having density 3.19 g/cm3. The compound decomposes at 1550°C. (ii) Magnesium orthosilicate: Mg2SiO4 [26686-77-1]; MW 140.69; occurs in nature as the mineral forsterite. It is a white crystalline solid consiting of orthorhombic crystals. It has a density 3.21 g/cm3 and melts at 1,898°C. (iii) Magnesium trisilicate: Mg2Si3O8; also known as magnesium mesotrisilicate; occurs in nature as minerals sepiolite, parasepiolite, and meerschaum. The compound is obtained as a fine white powder. Its pentahydrate occurs in nature as the mineral sellagen. (iv) Chrysotile [12001-29-5], a white serpentine fibrous silicate, is a major asbestos mineral. It is a tetrasilicate compound of magnesium, having the formula Mg6Si4O10(OH)8 containing (Si4O116–)n chain. (v) Complex silicates: magnesium silicate is a component of several complex silicates, including tremolite, an amphibole-type tetrasilicate Ca2Mg5(Si4O11)2 containing double-strand cross-linked (Si4O116–)n ; and diopside, a calcium magnesium metasilicate [CaMg(SiO3)2] consisting of pyroxene-type singlestrand chains of composition (Si4O32–)n. (vi) Talc [14807-96-6] or talcum: a very finely powdered hydrous magnesium silicate. Its formula is Mg3SiO10(OH)2 or 3MgO•4SiO2•HOH. It occurs in nature in compact and lump form, known as steatite or soapstone. The latter pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 535 MAGNESIUM SULFATE 535 is an impure variety of steatite. Talc is a white or grayish-white powder, density 2.7 g/cm3 and adheres readily to skin. Magnesium silicates have numerous applications in several industries, such as ceramics, glass, refractories, paints, rubber, chemicals, and food. Some general applications include manufacture of dry resins and resinous compositions; filler for rubber, paper and soap; bleaching agent for vegetable oils; anticaking agent in food; catalyst; pigment in paints and varnishes; dusting and shoe powder; toilet preparations; heat and electric insulators; and antacid and gastric sedative in medicine and a filler for pills. Florisil, a porous and granular form of activated magnesium silicate, is used for cleanup of sample extracts from interfering substances in gas chromatographic analysis. Thermochemical Properties (Mg2SiO4) ∆Hƒ° –519.6 kcal/mol ∆Gƒ° –491.2 kcal/mol S° 22.7 cal/degree mol Cρ 28.3 cal/degree mol Production Magnesium silicate occurs in nature in a variety of minerals, and is mined. The pyrosilicate is prepared by treating an aqueous solution of a magnesium salt with a solution of sodium silicate. The active form can be made by adjusting drying temperature and degree of hydration. Analysis Magnesium silicates are characterized by x-ray diffraction and Raman spectroscopy. Magnesium is analyzed in an aqueous acid extract by AA or ICP following digestion of the solid with nitric acid and appropriate dilution. MAGNESIUM SULFATE [7487-88-9] Formula: MgSO4; MW 120.36. Forms several stable hydrates, many of which occur in nature. The hydrates, their formulas, mineral names, and CAS Registry Numbers are tabulated below: Hydrate monohydrate tetrahydrate pentahydrate hexahydrate heptahydrate Mineral Name kieserite starkeyite pentahydrite hexahydrite epsomite Formula MgSO4•H2O MgSO4•4H2O MgSO4•5H2O MgSO4•6H2O MgSO4•7H2O CAS No. [14168-73-1] [24378-31-2] [15553-21-6] [13778-97-7] [10034-99-8] Occurrence and Uses Magnesium sulfate is found in nature in many salt deposits and mineral waters, occurring as hydrates or double salts. The heptahydrate or Epsom salt pp-03-25-new dots.qxd 536 10/23/02 2:38 PM Page 536 MAGNESIUM SULFATE was discovered in 1695, found in the mineral water at Epsom. Kieserite and epsomite are the two most important minerals. Other than these and the above hydrates, magnesium sulfate also is found in several other minerals, including: langbeinite, leonite vanthoffite bloedite kainite polyhalite K2SO4•2MgSO4 K2SO4•MgSO4•4H2O 3Na2SO4•MgSO4 Na2SO4•MgSO4•4H2O 4KCl•4MgSO4•11H2O [13826-56-7] [15226-80-9] [15557-33-2] [15083-77-9] [67145-93-1] K2SO4•MgSO4•2CaSO4•2H2O [15278-29-2]. Magnesium sulfate is used widely in several industries including fertilizer, cement, textile, chemicals, and medicine. In the cement industry, it is used in manufacturing oxysulfate cement. In medicine, it is an analgesic and cathartic. An important application of anhydrous magnesium sulfate in the laboratory involves drying organic solvents required for syntheses and GC analysis. In the textile industry, magnesium sulfate is used in finishing composition for dressing cotton; for weighting and sizing silk; as a mordant for fixing basic dyestuffs on wool; and in fireproofing fabrics. It also is a component of certain types of electrolytic plating baths; of various photographic solutions; of cosmetic lotions. It is a catalyst carrier; a dietary supplement in cattle feed; a coagulant for rubber and plastic; and is used in making citric acid and several magnesium salts, such as magnesium stearate. Physical Properties The anhydrous salt consists of colorless rhombohedral crystals; density 2.66 g/cm3; decomposes at 1,124°C; dissolves in water (269 g/100mL at 0°C), ethanol and glycerol; sparingly soluble in ether (1.16 g/mL at 18°C); insoluble in acetone. The monohydrate MgSO2•H2O, as the mineral kieserite, consists of colorless monoclinic crystals; refractive index 1.523; density 2.445 g/cm3; becomes anhydrous on heating at 200°C; soluble in water. Epsom salt, or heptahydrate MgSO2•7H2O, constitutes colorless monoclinic or rhombohedral crystals; refractive index 1.433; density 1.68 g/cm3; loses six molecules of water of crystallization at 150°C and converts to anhydrous form at 200°C; highly soluble in water (71 g/100mL at 20°C); slightly soluble in alcohol and glycerol. Thermochemical properties ∆Hƒ° (MgSO4) ∆Hƒ° (MgSO4•2H2O) ∆Hƒ° (MgSO4•4H2O) ∆Hƒ° (MgSO4•6H2O) ∆Hƒ° (MgSO4•7H2O) ∆Gƒ° ( MgSO4) ∆Gƒ° ( MgSO4•6H2O) –307.1 –453.2 –596.7 –737.8 –809.9 –279.8 –629.1 kcal/mol kcal/mol kcal/mol kcal/mol kcal/mol kcal/mol kcal/mol pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 537 MAGNESIUM SULFATE ∆Gƒ° ( MgSO4•7H2O) S° ( MgSO4) S° ( MgSO4•6H2O) S° ( MgSO4•7H2O) Cρ (MgSO4) Cρ (MgSO4•6H2O) 537 –686.4 kcal/mol 21.9 cal/degree mol 83.2 cal/degree mol 89.0 cal/degree mol 23.0 cal/degree mol 83.2 cal/degree mol Production Hydrated magnesium sulfate occurs in nature as the minerals kieserite and epsomite. The salt is mined in large scale from these and other naturally occurring minerals. The salt also is prepared in the laboratory by the action of sulfuric acid on magnesium oxide, hydroxide, or carbonate followed by evaporation and crystallization: MgO + H2SO4 → MgSO4 + H2O Mg(OH)2 + H2SO4 → MgSO4 + 2H2O MgCO3 + H2SO4 → MgSO4 + CO2 + H2O Crystallization at temperatures between 1.8 and 48°C yields heptahydrate, MgSO4•7H2O. Below 1.8°C, a dodecahydrate , MgSO4•12H2O crystallizes out. Above 48°C crystals of lower hydrates form. The anhydrous salt is obtained by heating the heptahydrate at about 500°C in a rotary drum; or dehydrating above 150°C in the presence of sulfuric acid. Reactions The anhydrous salt decomposes at elevated temperatures to magnesium oxide, oxygen, sulfur dioxide, and sulfur trioxide. The decomposition commences around 900°C and is complete at about 1,100°C. The overall reaction is: 900 −1100o C 3 MgSO4 → 3MgO + O2 +2SO2 + SO3 On the other hand, heating hydrated sulfate above 150°C yields magnesium oxysulfate, a hydrolysis reaction. No dehydration or thermal decomposition occurs. The anhydrous salt may be reduced to magnesium oxide when heated with carbon at 750°C: MgSO4 + C → MgO + SO2 + CO Magnesium sulfate undergoes three important types of reactions in aqueous solutions: double decomposition, double salt formation, and formation of oxysulfate cements. Many insoluble magnesium salts may be precipitated out by double decomposition reactions: pp-03-25-new dots.qxd 538 10/23/02 2:38 PM Page 538 MANGANESE MgSO4 + 2NaOH → Mg(OH)2 + 2Na+ + SO42– 3MgSO4 + 2Na3PO4 → Mg3(PO4)2 + 6Na+ +3 SO42– Magnesium sulfate forms several double salts having varying stoichiometric compositions. When gaseous ammonia is bubbled through magnesium sulfate solution, several hydrated double salts are obtained by crystallization. Magnesium sulfate double salts have the compositions MgSO4•NH3•3H2O; MgSO4•2NH3•4H2O; and MgSO4•2NH3•2H2O (Copp, A. N. 1981. Magnesium Compounds, In Kirk-Othmer Encyclopedia of Chemical Technology, 3rd ed., Vol. 14, pp. 636-40, New York: Wiley Interscience.) Similarly, in sulfuric acid, crystals of double salts MgSO4•H2SO4•3H2O, MgSO4•H2SO4, and MgSO4•3H2SO4 are obtained. Addition of magnesium oxide to magnesium sulfate solutions yields crystalline oxysulfates at varying stoichiometric compositions, such as MgSO4•3MgO•11H2O and MgSO4•5MgO•8H2O. Treatment of barium peroxide, BaO2 with a concentrated solution of magnesium sulfate yields magnesium peroxide MgO2, a white powdery material used as a bleaching and oxidizing agent, and as an antacid in medicine. Analysis Elemental composition (of anhydrous MgSO4) Mg 20.20%, S 26.63%, O 53.16%. The water of crystalization may be measured by thermogravimetric methods. Magnesium may be analyzed by AA or ICP-AES following acid digestion. MANGANESE [7439-96-5] Symbol: Mn; atomic number 25; atomic weight 54.938; a Group VIIB (Group 7) transition metal; electron configuration [Ar]4s23d7; atomic radius 1.27Å; valence 0, +1, +2, +3, +4, +5, +6, +7; most common oxidation states +2, +4 and +7; stable natural isotope Mn-55 (100%) History, Occurrence, and Uses Manganese was recognized as an element by Scheele, Bergman and others in 1774 and isolated by Gahn in the same year. Gahn obtained the metal by thermal reduction of pyrolusite with carbon. The element derived its name from the Latin word, magnes which means magnet, referring to the magnetic properties of its ore pyrolusite. Manganese is distributed widely in nature, mostly as oxide, silicate, and carbonate ores. Manganese ores often are found in association with iron ores in small quantities. The element, however, does not occur naturally in native form. Manganese is the twelfth most abundant element in the earth’s crust. pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 539 MANGANESE 539 Its concentration in the earth’s crust is estimated to be 0.095%. Its average concentration in seawater is 2µg/L. Manganese also is found in large quantities in deep-sea nodules over the ocean floor at depths of 2.5 to 4 miles. The composition of some common manganese minerals is tabulated below: Mineral Pyrolusite Manganite Hausmannite Rhodochrosite Rhodonite Bementite Braunite Psilomelane CAS Registry Number [14854-26-3] [52019-58-6] [1309-55-3] [598-62-9] [14567-57-8] [66733-93-5] — — — [12322-95-1] Composition MnO2 Mn2O3•H2O Mn3O4 MnCO3 MnSiO3 Mn8Si6O15(OH)10 3Mn2O3•MnSiO3 BaMnIIMnIV8O16(OH)4 Manganese is used widely in industry: the most important use is in ferrous metallurgy. It also is used in chemical, electrochemical, food and pharmaceutical applications. Ferromanganese alloys are used in steel manufacturing. Manganese serves as a deoxidizer of molten steel and controls its sulfur content. Manganese metal also enhances strength and hardness of the alloy, and its resistance to corrosion. Manganese is used in high-temperature steels, stainless steels, manganese steel and various nickel-chromium and manganese-aluminum alloys. Practically all aluminum and magnesium alloys contain manganese. Manganese is an essential element for plants and animals. Its shortage in soil can cause chlorosis or lack of chlorophyll in plants—manifested by the appearance of yellow or grey streaks on the leaves or mottling. It activates certain plant enzymes, such as oxalosuccinic decacarboxylase in the oxidation of carbohydrates. Manganese deficiency can cause deformity of bones in animals. In chemical industries, manganese is used to prepare several compounds. It also is used as a catalyst. Its salts have numerous applications in oxidation, catalysis, and medicine. Physical Properties Reddish-gray metal; exists in four allotropic modifications: alpha-, beta-, gamma- and delta forms. Alpha form has cubic crystal structure; 58 atoms per unit cell; density 7.43 g/cm3; brittle; transforms to beta form at 720°C. Betamanganese is brittle and has a cubic lattice structure; containing 20 atoms per unit cube; transforms to gamma form at 1,100°C or back to alpha form on cooling; density 7.29 g/cm3. The gamma form exists as face-centered cubic crystal containing 4 atoms per unit cell; density 7.18 g/cm3; converts to delta form at 1,136°C. Delta-manganese consists of body-centered cubic crystals containing 2 atoms per unit cube; density 6.30 g/cm3; stable up to 1,244°C above which it melts to liquid. Manganese vaporizes at 2,097°C; vapor pressure 0.9 torr at 1,244°C; hardness 5.0 (Mohs scale); magnetic susceptibility 9.9 cgs units at 18°C; electrical pp-03-25-new dots.qxd 540 10/23/02 2:38 PM Page 540 MANGANESE resistivities 185, 44, and 60 microhm–cm at 20°C for alpha-, beta- and gamma allotropes respectively; thermal neutron absorption 13.2 barns. Thermochemical Properties ∆Hƒ° (Mn-alpha) ∆Hƒ° (Mn-gamma) ∆Hƒ° (Mn-gas) ∆Gƒ° ( Mn-alpha) ∆Gƒ° ( Mn-gamma) ∆Gƒ° ( Mn-gas) S° ( Mn-alpha) S° (Mn-beta) S° ( Mn-gamma) S° (Mn-gas) Cρ (Mn-alpha) Cρ (Mn-beta) Cρ (Mn-gamma) Cρ (Mn-gas) ∆Hfus Coefficeint of linear expansion (at 25°C) 0.0 kcal/mol 0.37 kcal/mol 67.1 kcal/mol 0.0 kcal/mol 0.34 kcal/mol 57.0 kcal/mol 7.65 cal/degree mol 8.22 cal/degree mol 7.75 cal/degree mol 41.49 cal/degree mol 6.29 cal/degree mol 6.34 cal/degree mol 6.59 cal/degree mol 4.97 cal/degree mol 3.516 kcal/mol 22x10–6/°C Production Manganese is recovered primarily from its oxide ores, the most important being pyrolusite, MnO2. The basic method of producing the metal has not changed much since Gahn first isolated it by reducing manganese dioxide with carbon. Several processes to produce manganese meet its high demand in ferrous metallurgy. The oxides are reduced thermally in an electric furnace or a blast furnace. The ore is smelted at high temperatures in the presence of carbon, which reduces higher oxides of manganese, MnO2, Mn2O3, and Mn3O4 into MnO, and then forms metallic manganese which has a relatively high vapor pressure: MnO2 + C → MnO + CO Mn3O4 + C → 3MnO + CO MnO + C → Mn + CO Selection of the process depends on the requirement of the product, such as high-carbon or low-carbon ferromanganese or silicomanganese of varying carbon contents. Usually coke is used as a reducing agent for high-carbon ferromanganese for the steel industry. Low-carbon ferromanganese, silicomanganese, or refined ferromanganese that has low carbon content ranging from 0.1 to 1.5% maximum carbon, may be obtained by using silicon as a reducing agent: MnO2 + Si → Mn + SiO2 pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 541 MANGANESE 541 Mn3O4 + 2Si → 3Mn + SiO2 2MnO + Si → 2Mn + SiO2 Often, the manganese ores contain several other naturally occurring metal oxides such as alumina, silica, magnesia, and lime. Some of these oxides may be blended into manganese ore as fluxes to the furnace charge. Manganese may be produced by electrolytic processes. Aqueous solutions of manganese(II) sulfate are used as the electrolyte. Mn ore is roasted and reduced with carbon or silicon to convert the higher oxides of manganese into MnO. The products are then leached with dilute sulfuric acid at pH 3. MnO dissolves in the acid forming manganese(II) sulfate. The solution is filtered and separated from insoluble residues. It then is neturalized with ammonia to pH 6–7. Iron and aluminum precipitate out when treated with ammonia and are removed by filtration. Other metals, such as copper, zinc, lead and arsenic are precipitated and removed as sulfides upon passing hydrogen sufide through the solution. Colloidal particles of metallic sulfides and sulfur are removed by treatment with iron(II) sulfide. The purified solution of manganese(II) sulfate is then electrolyzed in an electrolytic cell using lead anode and Hastelloy or Type 316 stainless steel cathode, both of which are resistant to acid. Manganese is deposited on the cathode as a thin film. Manganese also is produced by electrolysis of fused salt. In one such process, the reduced MnO is blended to molten calcium fluoride and lime. The latter is used to neutralize silica in the ore. The fused composition of these salts is electrolyzed at 1,300°C in an electrolytic cell made up of high temperature ceramic material, using a carbon anode and a cathode consisting of iron bars internally cooled by water. Reactions Manganese forms compounds in several valence states: 0, +1, +2, +3, +4, +5, +6, and + 7. Of these, the valences 0, +1, and +5 are very uncommon. The divalent salts are the most stable. While in the divalent state, the metal is a reducing agent; in tetravalent state it is an oxidizing agent. Heptavalent manganese (Mn7+) is a powerful oxidizing agent. Some examples of Mn compounds in all these oxidation states are tabulated below: Oxidation State Mn(O) Mn(I) Mn(II) Mn(III) Mn(IV) Mn(V) Mn(VI) Mn(VII) Example Mn2(CO)10 C9H7Mn(CO)3 MnCl2; MnSO4; MnO MnF3; Mn2O3 MnO2; K2MnO3 K3MnO4 K2MnO4; BaMnO4 KMnO4; Mn2O7 pp-03-25-new dots.qxd 542 10/23/02 2:38 PM Page 542 MANGANESE Many chemical properties of manganese are similar to iron. Manganese burns in air or oxygen at elevated temperatures forming trimanganese tetroxide: 3Mn + 2O2 → Mn3O4 The metal reacts slowly with water in cold, forming manganous hydroxide with the evolution of hydrogen: Mn + 2H2O → Mn(OH)2 + H2 The reaction is usually slow below 100°C, but proceeds rapidly upon heating. Manganese reacts readily with dilute mineral acids forming their divalent salts and liberating hydrogen: Mn + 2HCl → MnCl2 + H2 Mn + H2SO4 → MnSO4 + H2 Manganese forms manganese(II) halides when heated with halogens. With fluorine, reaction is very vigorous and the products are MnF2 and MnF3: Mn + Cl2 → MnCl2 Mn + F2 → MnF2 2Mn + 3F2 → 2MnF3 When heated with sulfur, the product is manganese(II) sulfide, MnS2. Manganese combines with carbon or silicon at elevated temperatures forming a series of carbides or silicides having compositions such as Mn2C7, Mn3C, Mn7C3 and Mn15C4 or MnSi, Mn3Si and Mn5Si3. Manganese reacts with nitrogen above 750°C forming various nitrides, such as Mn3N2, Mn5N2 and Mn4N. The metal ignites in nitrogen at 1,200°C, then burns with a heavy, smoky flame forming the above nitrides. The principal product is Mn3N2. Also reaction with anhydrous ammonia above 350°C yields several nitrides of varying composition. Manganese dissolves in concentrated alkali in boiling solutions forming manganese(II) hydroxide and hydrogen. However, in the presence of excess oxygen or under oxygen pressure, the product is a manganate: 2Mn + 4KOH + 3O2 → 2K2MnO4 + 2H2O Reactions with concentrated acids are slow at room temperature, but rapid when heated. No hydrogen forms in concentrated acids. With concentrated sulfuric and nitric acids, sulfur dioxide and nitric oxide form: Mn + 2H2SO4 → MnSO4 + SO2 + 2H2O pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 543 MANGANESE(II) CARBONATE 543 Mn + 2HNO3 → MnNO3 + NO + 2H2O Manganese combines with several metals at elevated temperatures forming binary compounds in varying compositions. Such metals include Al, Zn, Ni, Sn, As, Sb, Be, Pd, and Au. Analysis Manganese in aqueous solution may be analyzed by several instrumental techniques including flame and furnace AA, ICP, ICP-MS, x-ray fluorescence and neutron activation. For atomic absorption and emission spectrometric determination the measurement may be done at the wavelengths 279.5, 257.61 or 294.92 nm respectively. The metal or its insoluble compounds must be digested with nitric acid alone or in combination with another acid. Soluble salts may be dissolved in water and the aqueous solution analyzed. X-ray methods may be applied for non-destructive determination of the metal. The detection limits in these methods are higher than those obtained by the AA or ICP methods. ICP-MS is the most sensitive technique. Several colorimetric methods also are known, but such measurements require that the manganese salts be aqueous. These methods are susceptible to interference. Manganese produces violet color in an oxidizing flame on a microcosmic or borax bead. The color disappears in a reducing flame. Toxicity Although trace amounts of manganese are essential for animals, in large quantities the metal can cause acute and chronic poisoning. Chronic inhalation of metal dust or fumes can cause manganism, a nonfatal disease affecting the central nervous system. The symptoms are mental disorder and disturbance in speech. MANGANESE(II) CARBONATE [598-62-9] Formula: MnCO3; MW 114.95 Synonyms: manganous carbonate; manganese spar; rhodochrosite Occurrence and Uses Manganese(II) carbonate occurs in nature as the mineral rhodochrosite [14476-12-1] (manganese spar). This ore also is used to produce manganese dioxide (by electrolytic process). The pure compound is used as gemstones; and as a pigment (manganese white). Physical Properties Pinkish-red translucent crystals; hexagonal-rhombohedral structure; refractive index 1.597; density 3.70 g/cm3; hardness 3.8 Mohs; decomposes above 200°C; slightly soluble in water; KSP2.24x10–11; soluble in dilute acids. pp-03-25-new dots.qxd 544 10/23/02 2:38 PM Page 544 MANGANESE(II) CARBONATE Thermochemical Properties ∆Hƒ° (cry) ∆Hƒ° (ppt) ∆Gƒ° (cry) ∆Gƒ° ( ppt) S° ( cry) S° (ppt) –214.0 kcal/mol –210.9 kcal/mol –195.9 kcal/mol –194.0 kcal/mol 20.5 cal/degree mol 27.0 cal/degree mol Preparation Manganese(II) carbonate is mined from its naturally occurring mineral rhodochrosite. The compound may be prepared in the laboratory as a palepink precipitate by adding sodium bicarbonate to a solution of manganese(II) salt saturated with carbon dioxide. The product obtained is monohydrate, MnCO3•H2O. However, if the carbon dioxide-saturated solution, together with the above monohydrate precipitate, is heated in the absence of atmosphere oxygen, the monohydrate MnCO3•H2O is converted into the anhydrous MnCO3. Reactions The dry carbonate decomposes on heating, forming manganese(II) oxide and CO2: MnCO3 → MnO + CO2 When heated above 330°C, MnO is partially oxidized by CO2, thus the decomposition products also contain MnO2 and CO. When heated in air, the carbonate yields Mn3O4: 6MnCO3 + O2 → 2Mn3O4 + 6CO2 When heated in oxygen, manganese(III) oxide forms: 4MnCO3 + O2 → 2Mn2O3 + 4CO2 Reaction with dilute acids forms manganese salts of the acids, liberating CO2: MnCO3 + H2SO4 → MnSO4 + CO2 + H2O Analysis Elemental composition: Mn 47.79%, C 10.45%, O 41.76%. The compound is dissolved in dilute HCl and CO2 liberated is identified by the lime water test (turns lime water milky), by GC-TCD, or GC/MS. The characteristic mass for CO2 is 44. The acid solution may be analyzed for Mn by AA, ICP or other instrumental technique (see Manganese). pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 545 MANGANESE(II) CHLORIDE 545 MANGANESE(II) CHLORIDE [7773-01-5] Formula: MnCl2; MW 125.84; forms a stable tetrahydrate, MnCl2•4H2O Synonyms: manganous chloride; manganese dichloride; scacchite Uses Manganese(II) chloride is used in dyeing and printing textiles and as a disinfectant. It also is used in dry cell batteries; for the preparation of drying agents for paints and varnishes; as a catalyst in chlorination reactions; in the production of several manganese salts, including methylcyclopentadienylmanganese tricarbonyl used as a colorant for brick. In metallurgy, the compound is used as an alloying agent and is added to molten magnesium to produce magnesium-manganese alloys. Physical Properties The anhydrous chloride is a pink solid; cubic crystals; deliquescent; density 2.977 g/cm3 at 25°C; melts at 650°C; vaporizes at 1,190°C; very soluble in water (~72g/100 mL at 25°C); soluble in alcohol; insoluble in ether. The tetrahydrate has a rose color; monoclinic crystal structure; deliquescent; density 2.01 g/cm3; melts at 58°C; loses one molecule of water at 106°C and all water at 198°C; highly soluble in water (151 g/100mL at 8°C) and extremely soluble in boiling water (656 g/100mL at 100°C); soluble in ethanol; insoluble in ether. Thermochemical Properties ∆Hƒ° (MnCl2) ∆Hƒ° (MnCl2•4H2O) ∆Gƒ° ( MnCl2) ∆Gƒ° (MnCl2•4H2O) S° (MnCl2) S° MnCl2•4H2O) Cρ (MnCl2) –115.0 kcal/mol –403.3 kcal/mol –105.3 kcal/mol –340.3 kcal/mol 28.26 cal/degree mol 72.5 cal/degree mol 17.43 cal/degree mol Preparation Manganese(II) chloride is prepared by heating manganese(II) oxide, manganese dioxide, manganese(II) carbonate or manganese(II) hydroxide with hydrochloric acid: MnO2 + 4HCl → MnCl2 + 2H2O + Cl2 MnCO3 + HCl → MnCl2 + H2O + CO2 When the product mixture is evaporated below 58°C, the tetrahydrate salt, MnCl2•4H2O is obtained. Manganese(II) chloride is a by-product in the manufacture of chlorine from manganese dioxide and hydrochloric acid (the Weldon process). pp-03-25-new dots.qxd 546 10/23/02 2:38 PM Page 546 MANGANESE DECACARBONYL Anhydrous chloride can be prepared by heating manganese(II) oxide or manganese(II) carbonate with dry hydrogen chloride; or by burning the metal in chlorine at 700°C to 1,000°C. The anhydrous salt can also be obtained by slowly heating the tetrahydrate, MnCl2•4H2O in a rotary drier above 200°C or by dehydration in a stream of hydrogen chloride gas. Reactions Manganese(II) chloride forms double salts with alkali metal chlorides when mixed in stoichiometric amounts. Such double salts, which can decompose in water, may have compositions like KMnCl3 or K2MnCl4. Manganese(II) chloride forms adducts with ammonia, hydroxylamine and many other nitrogen compounds. Many adducts are stable at ordinary temperatures. Examples are MnCl2•6NH3 and MnCl2•2NH2OH. An aqueous solution can readily undergo double decomposition reactions with soluble salts of other metals, producing precipitates of insoluble salts of Mn(II) or other metals. Analysis Elemental composition: Mn 43.66%, Cl 56.34% An aqueous solution of the compound may be analyzed for Mn by AA, ICP, or other instrumental techniques, and for chloride by ion chromatography or titration against a standard solution of silver or mercuric nitrate. MANGANESE DECACARBONYL [10170-69-1] Formula: Mn2(CO)10; MW 389.99; manganese in zero oxidation state. Synonyms: dimanganese decacarbonyl; manganese carbonyl Uses Manganese decacarbonyl is used as an antiknock additive to gasoline; and as a catalyst. Physical Properties Golden-yellow monoclinic crystals; density 1.75 g/cm3; melts at 154 to 155°C; decomposition commences around 110°C, slowly losing carbon monoxide; stable under carbon monoxide atmosphere; insoluble in water; soluble in most organic solvents. Preparation Manganese decacarbonyl is prepared by the reduction of methylcyclopentadienylmanganese tricarbonyl (MMT) with sodium in diglyme under carbon monoxide pressure. Alternatively, the compound can be prepared by reduction of manganese(II) iodide with a Grignard reagent in the presence of carbon monoxide under pressure. pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 547 MANGANESE ETHYLENENEBIS(THIOCARBAMATE) 547 Analysis Elemental composition: Mn 28.17%, C 30.80%, O 41.03%. The compound is cautiously digested with nitric acid, diluted and analyzed for manganese by instrumental techniques. Its solution in an organic solvent may be analyzed by GC/MS. Toxicity The compound is toxic by ingestion and possibly by other routes of exposure. MANGANESE ETHYLENENEBIS(THIOCARBAMATE) [12427-38-2] Formula: C4H6MnN2S4; MW 256.29 Structure: CH2NHC(=S)—S Mn CH2NHC(=S)—S Synonyms: Maneb; [ethylenebis(dithiocarbamato)]manganese; manganous ethylenebis(dithiocarbamate) Uses The compound is a fungicide. Physical Properties Yellow powder; crystallizes from methanol or ethanol; melts between 192° to 204°C; low solubility in water; soluble in chloroform and pyridine. Preparation Manganese ethylenebis(thiocarbamate) is made by adding disodium ethylenebis(dithiocarbamate) (also, known as Nabam, commercially available) to an aqueous solution of manganese(II) sulfate: NaSC(=S)NHCH2CH2NHC(=S)SNa + MnSO4 → C4H6MnN2S4 + Na2SO4 Alternatively, the compound may be prepared by neutralizing an aqueous solution of disodiummethylenebis(dithiocarbamate) (Nabam) with acetic acid followed by addition of manganese(II) chloride solution. pp-03-25-new dots.qxd 548 10/23/02 2:38 PM Page 548 MANGANESE(II) HYDROXIDE Analysis Elemental composition: Mn 20.70%, S 48.35%, C 18.11%, N 10.56%, H 2.28%. A chloroform solution of the compound may be analyzed by GC/MS or by GC-FPD. Manganese may be determined by digesting the compound with nitric acid and analyzing the diluted acid extract by AA or ICP. Toxicity Maneb is toxic by ingestion. MANGANESE(II) HYDROXIDE [18933-05-6] Formula: Mn(OH)2; MW 88.953 Synonyms: manganous hydroxide; pyrochroite Occurrence: Manganese(II) hydroxide occurs naturally as the mineral pyrochroite Physical Properties Pink hexagonal crystal; density 3.26 g/cm3; refractive index 1.68; Mohs hardness 2.5; decomposes at 140°C; insoluble in water; KSP 5.61x10–12; soluble in acid; dissolves in alkaline solution on heating. Thermochemical Properties ∆Hƒ° –167.0 kcal/mol ∆Gƒ° –148.0 kcal/mol S° 23.0 cal/degree mol Preparation Manganese(II) hydroxide is obtained as a white precipitate by adding a solution of sodium or potassium hydroxide to a solution of manganese(II) salt, such as manganese(II) chloride: Mn2+ + 2OH¯ → Mn(OH)2 The white precipitate rapidly turns brownish-pink in air. The reaction does not occur with ammonia in the presence of ammonium salt. The hydroxide also is found in nature as mineral pyrochroite in the form of white transparent leaflets. The white leaflets turn pink on exposure to air. Reactions Manganese(II) hydroxide is a base exhibiting weak amphoteric behavior. It reacts with acids forming the corresponding manganese(II) salt: Mn(OH)2 + 2KOH → K2Mn(OH)4 The hydroxide is rapidly oxidized in air forming manganese(III) oxide, Mn2O3. pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 549 MANGANESE(II) OXIDE 549 Analysis Elemental composition: Mn 61.76%, H 2.27%, O 35.97%. The compound is digested in nitric acid and analyzed for manganese by AA, ICP or other instrumental technique. MANGANESE(II) OXIDE [1344-43-0] Formula: MnO; MW 70.94 Synonyms: manganous oxide; manganese monoxide; green manganese oxide; manganosite [1313-12-8] Occurrence and Uses Manganese(II) oxide occurs naturally as manganosite [1313-12-8]. The mineral is found very rarely in nature. Manganese(II) oxide is used in the fertilizer industry as a source of manganese in fertilizers; in feedstuff formulations; and as an intermediate in the production of several manganese compounds. Physical Properties Green cubic crystal; refractive index 2.16; density 5.37 g/cm3 at 23°C; Moh’s hardness 5.5; melts at 1945°C; insoluble in water. Thermochemical Properties ∆Hƒ° ∆Gƒ° S° Cρ –92.07 kcal/mol –86.74 kcal/mol 14.27 cal/degree mol 10.86 cal/degree mol Production Manganese(II) oxide is obtained commercially from manganese(IV) oxide (manganese dioxide) by the reduction with hydrogen, carbon monoxide or methane at elevated temperatures (>800°C): MnO2 + CO → MnO + CO2 MnO2 + H2 → MnO + H2O The oxide also can be made by thermal decomposition of manganese(II) carbonate or manganese(II) oxalate in the absence of air: MnCO3 → MnO + CO2 Also, careful dehydration of manganese(II) hydroxide, Mn(OH)2, under controlled conditions in the absence of air yields MnO. pp-03-25-new dots.qxd 550 10/23/02 2:38 PM Page 550 MANGANESE(III) OXIDE Reactions Manganese(II) oxide is the lowest oxide of manganese and it is purely a basic oxide. It reacts with acids to form their manganese(II) salts: MnO + H2SO4 → MnSO4 + H2O MnO + 2HCl → MnCl2 + H2O The compound also is oxidized by air or oxygen to higher oxides of manganese. When heated cautiously in air, the product is manganese sesquioxide or manganese(III) oxide: 4MnO + O2 → 2Mn2O3 Analysis Elemental composition: Mn 77.44%, O 22.55%. The oxide can be characterized nondestructively by x-ray methods. Also, manganese may be analyzed by AA or ICP technique following acid digestion with nitric acid and diluting the acid extract appropriately (see Manganese). MANGANESE(III) OXIDE [1317-34-6] Formula: Mn2O3; MW 157.87 Synonyms: manganese sesquioxide; dimanganese trioxide Occurrence and Uses Manganese(III) oxide occurs in nature as the mineral braunite. The oxide is used in the production of ferrites and thermistors. Physical Properties Black cubic (or rhombic) crystals; density 4.50 g/cm3; Moh’s hardness 6–6.5 (for braunite); decomposes at about 875°C; insoluble in water; insoluble in alcohol and acetone; soluble in acids. Thermochemical Properties ∆Hƒ° ∆Gƒ° S° Cρ –229.2 kcal/mol –210.6 kcal/mol 26.40 cal/degree mol 25.73 cal/degree mol Preparation Manganese(III) oxide is obtained by heating manganese(II) oxide in air at 600 to 850°C. It also may be prepared by igniting manganese(II) salts in air pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 551 MANGANESE(II,III) OXIDE 551 or oxygen. The oxide also is produced by cautious heating of manganese(II) oxide in oxygen. Manganese(III) oxide also can be made by dehydrating manganese(III) metahydroxide, MnO(OH), in a vacuum at 250°C. In such preparation, an unstable tetragonal modification, beta-Mn2O3, is first obtained which on prolonged heating converts to the stable cubic modification, alphaMn2O3. Analysis Elemental composition: Mn 69.59%, O 30.41%. The oxide can be characterized by x-ray methods and analyzed for manganese by AA or ICP following acid extraction. MANGANESE(II,III) OXIDE [1317-35-7] Formula: Mn3O4; MW 228.81 Synonyms: trimanganese tetraoxide; manganomanganic oxide; red oxide of manganese Occurrence and Use Manganese(II,III) oxide occurs in nature as the mineral hausmannite [1309-55-3]. It is used to make ferrites and thermistors. The oxide also is used in the thermite process for producing manganese. Physical Properties Black tetragonal crystal; exhibits two allotropic modifications—a stable alpha phase, occurring in tetragonal crystalline form (as hausmannite) and an unstable beta modification; density 4.85 g/cm3; Moh’s hardness 5.5; melts at 1,567°C; insoluble in water; soluble in hydrochloric acid. Thermochemical Properties ∆Hƒ° ∆Gƒ° S° Cρ –331.7 kcal/mol –306.7 kcal/mol 37.2 cal/degree mol 33.4 cal/degree mol Preparation Manganese(II,III) oxide is made by heating manganese(IV) oxide, MnO2, or manganese(III) oxide, Mn2O3, above 950°C. When Mn2O3 is heated in air, the temperature should be above 940°C, but if heated in oxygen, the temperature should be above 1,090°C. Also, heating manganese(III) oxide at 230°C in hydrogen yields Mn3O4. However, further heating above 300°C converts Mn3O4 formed to green manganese(II) oxide, MnO. Manganese(II,III) oxide also is obtained by heating the dioxide, MnO2, with carbon at 600 to 700°C. pp-03-25-new dots.qxd 552 10/23/02 2:38 PM Page 552 MANGANESE(IV) OXIDE Reactions Manganese(II,III) oxide reacts with dilute acids forming the corresponding manganous salt and manganese(IV) oxide, MnO2: Mn3O4 + 2H2SO4 → 2MnSO4 + MnO2 + 2H2O The oxide, however, dissolves slowly in cold sulfuric acid forming a red solution that also contains manganic sulfate, Mn2(SO4)3: Mn3O4 + 4H2SO4 → MnSO4 + Mn2(SO4)3 + 4H2O Reaction with acetic acid yields manganese(II) acetate and manganese(III) oxide: Mn3O4 + 2CH3COOH → Mn(CH3COO)2 + Mn2O3 + H2O Manganese(II,III) oxide is reduced to manganese metal when heated with powdered aluminum (the Thermite process). The reaction is vigorous and exothermic: 3Mn3O4 + 8Al → 4Al2O3 + 9Mn Analysis Elemental composition: Mn 72.03%, O 27.98%. The oxide can be characterized by x-ray methods. Manganese in the oxide can be analyzed by AA or ICP method after digesting the oxide in nitric acid. MANGANESE(IV) OXIDE [1313-13-9] Formula: MnO2; MW 86.937 Synonyms: manganese dioxide; manganese peroxide; black manganese oxide Occurrence and Uses Manganese(IV) oxide is the most important ore of manganese from which the metal is mostly manufactured. The oxide occurs in nature as the mineral pyrolusite as heavy gray lumps, or black when powdered. The mineral is used to produce manganese metal, most manganese salts, and also manganese steel and other alloys. The metallurgical applications of manganese(IV) oxide mainly involve making ferromanganese and special manganese alloys. Another important application of manganese(IV) oxide is in manufacturing dry-cell batteries and alkaline cells. The oxide also is a colorant in brick, tile, porcelain and glass; a drier for paints and varnishes; a pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 553 MANGANESE(IV) OXIDE 553 preparation for printing and dyeing textiles; a curing agent for polysulfide rubbers; an adsorbent for hydrogen sulfide and sulfur dioxide; an oxidizing agent in many organic syntheses such as quinone and hydroquinone; and a catalyst in laboratory preparation of oxygen from potassium chlorate. Manganese(IV) oxide also is used to make welding rods and fluxes, and ceramic magnets (ferrites); and is an additive to fertilizers. Physical Properties Black tetragonal crystals; density 5.08 g/cm3; Moh’s hardness 6.3; decomposes at 535°C; insoluble in water. Thermochemical Properties ∆Hƒ° ∆Gƒ° S° Cρ –124.3 kcal/mol –111.2 kcal/mol 12.69 cal/degree mol 12.93 cal/degree mol Preparation Pure manganese(IV) oxide (precipitate form) may be prepared by reducing permanganate ion with a manganous salt: 2KMnO4 + 3MnSO4 + 2H2O → 5MnO2 + K2SO4 + 2H2SO4 Manganese(IV) oxide can also be precipitated by oxidation of a manganese(II) salt using an oxidizing agent such as hypochlorite or peroxydisulphate: Mn2+ + S2O82– + 2H2O → MnO2 + 2SO42– + 4H+ Manganese(IV) oxide may also be made by thermal decomposition of manganese(II) nitrate; or from roasting manganese(II) carbonate in air: Mn(NO3)2 → MnO2 + 2NO2 MnCO3 + ½ O2 → MnO2 + CO2 A highly active gamma-MnO2 can be produced by treating manganese(III) oxide with hot sulfuric acid: Mn2O3 + H2SO4 → MnO2 + MnSO4 + H2O Mn2O3 is derived from pyrolusite by heating the mineral at 600–800°C or reducing with powdered coal at 300°C. Reactions Thermal decomposition of manganese(IV) oxide at 600 to 800°C yields manganese(III) oxide: pp-03-25-new dots.qxd 554 10/23/02 2:38 PM Page 554 MANGANESE(IV) OXIDE 4MnO2 → 2Mn2O3 + O2 MnO2 also is reduced to Mn2O3 at 300°C in the presence of a reducing agent such as hydrogen, methane or carbon. Treatment with concentrated hydrochloric acid forms manganese(IV) chloride which readily decomposes to manganese(III) chloride and manganese(II) chloride, successively liberating chlorine: MnO2 + 4HCl → MnCl4 + 2H2O MnCl4 → MnCl3 + ½ Cl2 MnCl3 → MnCl2 + ½ Cl2 When heated with concentrated sulfuric acid, manganese(IV) oxide yields manganese(II) sulfate, evolving oxygen: MnO2 + H2SO4 → MnSO4 + H2O + ½ O2 When the solution is heated at 135°C, MnSO4 is oxidized to Mn2(SO4)3. Reaction with sulfuric acid in the presence of oxalic acid yields manganese(II) sulfate and carbon dioxide: MnSO2 + (COOH)2 + H2SO4 → MnSO4 + 2CO2 + 2H2O While the reaction with sulfuric acid in the presence of sodium chloride evolves chlorine: MnO2 + 2NaCl + 2H2SO4 → MnSO4 + Na2SO4 + 2H2O + Cl2 When heated with potassium hydroxide, manganese(IV) oxide partially decomposes to manganese(III) oxide and potassium manganate: 3MnO2 + 2KOH → Mn2O3 + K2MnO4 + H2O However, in the presence of oxygen or other oxidizing agents, all manganese is oxidized to manganate: MnO2 + 2KOH + ½ O2 → K2MnO4 + H2O Manganate(VI) can further oxidize to manganate(VII) (or permanganate) in alkaline solution with a strong oxidizing agent such as hypochlorite, chlorine or perchlorate, or under anodic oxidation. Alternatively, in less alkaline media (where the KOH concentration is less than about 15%), the manganate ion MnO42– hydrolyzes, disproportionating to permanganate MnO4¯ and forming back manganese(IV) oxide: pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 555 MANGANESE(IV) OXIDE 555 3MnO42– + 2H2O → 2MnO4¯ + MnO2 + 4OH¯ The green color of manganate solution turns purple due to the permanganate formed. Manganese(IV) oxide is an oxidizing agent. In acid medium, it oxidizes iodide to iodine: MnO2 + 2I¯ + 4H+ → Mn2+ + 2H2O + I2 Thus, in the presence of dilute acids, MnO2 is readily attacked by strong reducing agents. Similarly, reaction with sulfurous acid forms manganese(II) dithionate: MnO2 + 2H2SO3 → MnS2O6 + 2H2O Or with nitrous acid in the presence of nitric acid, manganese(II) nitrate is formed: MnO2 + HNO2 + HNO3 → Mn(NO3)2 + H2O Reaction with potassium bifluoride in the presence of hydrofluoric acid creates a stable complex fluoride, K2MnF6 in which Mn is in +4 oxidation state: MnO2 + 2KHF2 + 2HF → K2MnF6 + 2H2O When fused with basic oxides such as calcium oxide, manganites or manganate(IV) salts such as CaO•MnO2, 2CaO•MnO2, CaO•3MnO2 are formed. The stoichiometric compositions of these manganites vary. Manganese(IV) oxide reacts with aniline in the presence of sulfuric acid forming quinone, an intermediate product in the manufacture of hydroquinone: 4MnO2 + 2C6H5NH2 + 5H2SO4 → 2C6H4O2 + 4MnSO4 + (NH4)2SO4 + 4H2O Analysis Elemental composition: Mn 63.19%, O 36.81%. The pure oxide may be characterized by x-ray crystallography. The MnO2 content in pyrolusite may be measured by titration. An excess of a standard solution of oxalic acid is added to a solution of MnO2 in sulfuric acid. After all solid MnO2 dissolves, the excess oxalic acid is measured by titrating against a standard solution of potassium permanganate (see Reactions). Alternatively, pyrolusite is heated with concentrated hydrochloric acid and pp-03-25-new dots.qxd 556 10/23/02 2:38 PM Page 556 MANGANESE(II) SULFATE the chlorine evolved is passed through a solution of potassium iodide. The iodine liberated is titrated against a standard solution of sodium thiosulfate using starch indicator. One mol MnO2 is equivalent to two mol thiosulfate. Also, acid extracts of MnO2 may be diluted and measured by AA or ICP techniques (See Manganese). MANGANESE(II) SULFATE [7785-87-7] Formula: MnSO4; MW 151.00; forms stable monohydrate, MnSO4•H2O [10034-96-5] and tetrahydrate, MnSO4•4H2O [10101-68-5] Synonym: manganous sulfate Uses Manganese(II) sulfate is used to produce manganese by an electrolytic process. The compound is used for dyeing textiles; for producing red glazes on porcelain; in varnish driers; in fertilizers; and in animal feeds to provide manganese as an essential trace element. Physical Properties The anhydrous salt is a white orthogonal crystal; density 3.25 g/cm3; melts at 700°C; decomposes at 850°C; very soluble in water. The monohydrate MnSO4•H2O consists of red monoclinic crystals; density 2.95 g/cm3; highly soluble in water. The tetrahydrate MnSO4•4H2O is a pink solid; monoclinic crystals; density 2.107 g/cm3; highly soluble in water; more soluble than the anhydrous salt or the monohydrate. Thermochemical Properties ∆Hƒ° (MnSO4) ∆Hƒ° (MnSO4•H2O) ∆Hƒ° (MnSO4•4H2O) ∆Gƒ° (MnSO4) S° ( MnSO4) Cρ (MnSO4) –254.60 kcal/mol –329.00 kcal/mol –539.70 kcal/mol –228.83 kcal/mol 26.8 cal/degree mol 24.0 cal/degree mol Preparation Manganese(II) sulfate is prepared by prolonged heating of any manganese salt with concentrated sulfuric acid. The compound is produced commercially from pyrolusite (MnO2) or rhodochrosite (MnCO3). Either mineral is dissolved in sulfuric acid and the solution evaporated: MnO2 + H2SO4 → MnSO4 + H2O + ½ O2 Alternatively, manganese dioxide is heated strongly with dehydrated iron(II) pp-03-25-new dots.qxd 10/23/02 2:38 PM Page 557 MANGANESE(II) SULFATE 557 sulfate: 2MnO2 + 2FeSO4 → 2MnSO4 + Fe2O3 + ½ O2 Manganese(II) sulfate, prepared by methods involving evaporation of manganese salt with sulfuric acid, is the tetrahydrate, MnSO4•4H2O. The tetrahydrate on gentle heating produces monohydrate, MnSO4•H2O. Also, manganese(II) sulfate is a by-product in the manufacture of hydroquinone. The process involves reaction of aniline with manganese dioxide in sulfuric acid, followed by the removal of quinone by steam distillation under vacuum. 2C6H5NH2 + 5H2SO4 + 4MnO2 → 2C6H4O2 + 4MnSO4 + 2C6H4O2 + 4MnSO4 (aniline) (quinone) The unreacted acid is neutralized by lime, treated with water, and the solution filtered to separate any excess MnO2 and insoluble residues. Evaporation of the filtrate yields a crude product containing about 80% MnSO4 and 15% (NH4)2SO4. Manganese(II) sulfate also may be produced by the action of sulfur dioxide with manganese dioxide: MnO2 + SO2 → MnSO4 Reactions Aqueous solution of manganese(II) sulfate undergoes double decomposition reactions precipitating insoluble manganese(II) salts; for example, adding caustic soda solution precipitates manganese(II) hydroxide. Manganese(II) sulfate forms several double salts, such as manganese(II) ammonium sulfate, (NH4)2Mn(SO4)2•6H2O. Reaction with oxalic acid, stearic acid, phthalic acid or their alkali salts yield their corresponding manganese salts (manganese soaps). Manganese(II) sulfate may be oxidized electrolytically to manganese dioxide (gamma form) in an electrolytic cell. MnSO4 + 2H2O → MnO2 + H2SO4 + H2 Manganous(II) sulfate is a reducing agent. Treatment with oxidizing agents can yield manganese compounds in a higher oxidation state. Analysis Elemental composition: Mn 36.38%, S 21.23%, O 42.38%. Manganese may be analyzed in an aqueous solution of the compound by AA, ICP or x-ray fluorescence methods. Sulfate can be determined by ion chromatography. Water of crystallization in hydrated sulfate may be measured by heating at 400°C (by gravimetry).